#------------------------------------------------------------------------------
#$Date: 2021-04-12 10:25:35 +0300 (Mon, 12 Apr 2021) $
#$Revision: 264046 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/16/1561643.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1561643
loop_
_publ_author_name
'Ortner, Teresa S.'
'Wurst, Klaus'
'Hejny, Clivia'
'Huppertz, Hubert'
_publ_section_title
;
 Hydrothermal synthesis and characterization of the lutetium
 borate--nitrate Lu2B2O5(NO3)2·2H2O
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              329
_journal_page_last               334
_journal_paper_doi               10.1016/j.jssc.2015.11.005
_journal_volume                  233
_journal_year                    2016
_chemical_formula_moiety         'B4 H8 Lu4 N4 O26'
_chemical_formula_sum            'B4 H8 Lu4 N4 O26'
_chemical_formula_weight         1223.22
_chemical_name_common            'Lutetiumdiborate-nitrate dihydrate'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                90.825(2)
_cell_angle_beta                 101.748(2)
_cell_angle_gamma                110.018(2)
_cell_formula_units_Z            2
_cell_length_a                   7.8952(5)
_cell_length_b                   9.8862(6)
_cell_length_c                   14.6033(8)
_cell_measurement_reflns_used    9674
_cell_measurement_temperature    120(2)
_cell_measurement_theta_max      35.3
_cell_measurement_theta_min      2.7
_cell_volume                     1044.15(11)
_computing_cell_refinement       'Bruker SAINT-V 8.34A'
_computing_data_collection       'Bruker Apex II'
_computing_data_reduction        'Bruker SAINT-V 8.34A'
_computing_molecular_graphics
'DIAMOND Version 3.2i(Brandenburg & Putz, 2012)'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    SHELXTL-2013/1
_diffrn_ambient_temperature      120(2)
_diffrn_detector_area_resol_mean 10.4
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker D8 Quest'
_diffrn_measurement_method       'phi- and omega-scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0498
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            52874
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         34.998
_diffrn_reflns_theta_min         2.202
_diffrn_source                   'Incoatec Microfocus'
_exptl_absorpt_coefficient_mu    18.878
_exptl_absorpt_correction_T_max  0.645
_exptl_absorpt_correction_T_min  0.425
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Bruker DIFABS-2014/5'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.891
_exptl_crystal_description       plate
_exptl_crystal_F_000             1096
_exptl_crystal_size_max          0.06
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.02
_refine_diff_density_max         11.394
_refine_diff_density_min         -4.045
_refine_diff_density_rms         0.478
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.066
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     344
_refine_ls_number_reflns         9176
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.066
_refine_ls_R_factor_all          0.0639
_refine_ls_R_factor_gt           0.0439
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0514P)²+15.2065P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0996
_refine_ls_wR_factor_ref         0.1086
_reflns_number_gt                7279
_reflns_number_total             9176
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            JSSC-2016-233-329.cif
_cod_data_source_block           p
_cod_database_code               1561643
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_disorder_assembly
_atom_site_disorder_group
Lu1 Lu 0.03776(5) 0.44541(3) 0.89336(2) 0.01576(7) Uani 1 d . .
Lu2 Lu -0.02720(4) 1.02346(3) 0.87559(2) 0.01126(6) Uani 1 d . .
Lu3 Lu -0.01500(4) 0.52972(3) 0.61947(2) 0.01178(6) Uani 1 d . .
Lu4 Lu 0.05077(4) 0.94876(3) 0.61312(2) 0.01222(6) Uani 1 d . .
B1 B -0.0161(11) 0.7515(8) 0.9341(5) 0.0139(13) Uani 1 d . .
B2 B 0.0257(12) 0.7070(8) 0.7697(5) 0.0148(13) Uani 1 d . .
B3 B -0.0034(12) 0.1983(8) 0.7346(5) 0.0148(13) Uani 1 d . .
B4 B 0.0208(11) 0.2624(8) 0.5685(5) 0.0121(12) Uani 1 d . .
N1 N 0.4245(12) 0.5616(11) 0.9112(7) 0.042(2) Uani 1 d . .
N2 N -0.4181(10) 0.9091(9) 0.8326(5) 0.0299(16) Uani 1 d . .
N3 N -0.4103(10) 0.4270(8) 0.5906(5) 0.0274(14) Uani 1 d . .
N4 N 0.4416(11) 1.0451(10) 0.6496(6) 0.0341(18) Uani 1 d . .
O1 O 0.0109(8) 0.7915(5) 0.8433(3) 0.0152(9) Uani 1 d . .
O2 O -0.0211(8) 0.6222(5) 0.9636(3) 0.0171(10) Uani 1 d . .
O3 O -0.0356(7) 0.8593(5) 0.9847(3) 0.0141(9) Uani 1 d . .
O4 O 0.0207(8) 0.5698(5) 0.7756(3) 0.0182(10) Uani 1 d . .
O5 O 0.0386(7) 0.7592(5) 0.6849(3) 0.0150(9) Uani 1 d . .
O6 O 0.0090(7) 0.2923(5) 0.6624(3) 0.0137(9) Uani 1 d . .
O7 O -0.0280(8) 0.2379(5) 0.8185(3) 0.0199(11) Uani 1 d . .
O8 O 0.0024(8) 0.0633(5) 0.7257(3) 0.0193(10) Uani 1 d . .
O9 O 0.0259(8) 0.3752(5) 0.5162(3) 0.0154(9) Uani 1 d . .
O10 O 0.0236(8) 0.1353(5) 0.5374(3) 0.0164(9) Uani 1 d . .
O13 O 0.5877(14) 0.6110(15) 0.9156(11) 0.092(5) Uani 1 d . .
O12 O 0.3424(12) 0.6239(9) 0.9532(6) 0.0459(19) Uani 1 d . .
O11 O 0.3232(12) 0.4403(10) 0.8671(7) 0.048(2) Uani 1 d . .
O16 O -0.5866(10) 0.8607(12) 0.8114(7) 0.059(3) Uani 1 d . .
O15 O -0.3218(10) 0.8601(8) 0.7928(5) 0.0372(16) Uani 1 d . .
O14 O -0.3273(10) 1.0130(9) 0.8946(5) 0.0408(18) Uani 1 d . .
O17 O -0.3137(11) 0.5460(9) 0.6350(7) 0.051(2) Uani 1 d . .
O19 O -0.5795(10) 0.3836(10) 0.5718(7) 0.050(2) Uani 1 d . .
O18 O -0.3220(11) 0.3593(9) 0.5596(7) 0.049(2) Uani 1 d . .
O22 O 0.6095(11) 1.0838(12) 0.6682(8) 0.065(3) Uani 1 d . .
O21 O 0.3406(10) 0.9433(10) 0.5885(5) 0.0416(18) Uani 1 d . .
O20 O 0.3571(11) 1.1031(9) 0.6941(6) 0.047(2) Uani 1 d . .
O23 O -0.2864(10) 0.3588(8) 0.8477(5) 0.0349(15) Uani 1 d . .
O24 O 0.2923(9) 1.0996(8) 0.9069(5) 0.0315(14) Uani 1 d . .
O25 O 0.3016(9) 0.6067(7) 0.6572(5) 0.0313(14) Uani 1 d . .
O26 O -0.2717(9) 0.8615(7) 0.5803(5) 0.0284(13) Uani 1 d . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0 0 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.006 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Lu Lu -0.472 5.8584 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 Lu1 O7 98.65(18) . .
O4 Lu1 O2 158.62(17) . 2_567
O7 Lu1 O2 99.77(18) . 2_567
O4 Lu1 O2 82.61(17) . .
O7 Lu1 O2 156.1(2) . .
O2 Lu1 O2 76.16(19) 2_567 .
O4 Lu1 O23 83.7(2) . .
O7 Lu1 O23 76.4(2) . .
O2 Lu1 O23 90.2(2) 2_567 .
O2 Lu1 O23 80.1(2) . .
O4 Lu1 O11 88.6(3) . .
O7 Lu1 O11 74.4(3) . .
O2 Lu1 O11 106.8(3) 2_567 .
O2 Lu1 O11 129.4(3) . .
O23 Lu1 O11 148.3(3) . .
O4 Lu1 O12 86.6(3) . .
O7 Lu1 O12 127.0(3) . .
O2 Lu1 O12 90.9(3) 2_567 .
O2 Lu1 O12 76.8(3) . .
O23 Lu1 O12 155.9(3) . .
O11 Lu1 O12 52.9(3) . .
O4 Lu1 N1 86.0(2) . .
O7 Lu1 N1 100.8(3) . .
O2 Lu1 N1 101.0(2) 2_567 .
O2 Lu1 N1 103.0(3) . .
O23 Lu1 N1 168.8(3) . .
O11 Lu1 N1 26.4(3) . .
O12 Lu1 N1 26.5(3) . .
O4 Lu1 Lu1 120.43(12) . 2_567
O7 Lu1 Lu1 133.71(14) . 2_567
O2 Lu1 Lu1 38.30(12) 2_567 2_567
O2 Lu1 Lu1 37.86(12) . 2_567
O23 Lu1 Lu1 83.83(17) . 2_567
O11 Lu1 Lu1 126.0(2) . 2_567
O12 Lu1 Lu1 82.2(2) . 2_567
N1 Lu1 Lu1 105.3(2) . 2_567
O4 Lu1 N1 126.2(2) . 2_667
O7 Lu1 N1 95.1(2) . 2_667
O2 Lu1 N1 62.66(19) 2_567 2_667
O2 Lu1 N1 103.4(2) . 2_667
O23 Lu1 N1 150.1(2) . 2_667
O11 Lu1 N1 46.2(3) . 2_667
O12 Lu1 N1 45.5(2) . 2_667
N1 Lu1 N1 40.2(3) . 2_667
Lu1 Lu1 N1 81.82(14) 2_567 2_667
O4 Lu1 N3 41.46(18) . .
O7 Lu1 N3 73.17(17) . .
O2 Lu1 N3 136.73(18) 2_567 .
O2 Lu1 N3 93.49(16) . .
O23 Lu1 N3 46.5(2) . .
O11 Lu1 N3 111.8(2) . .
O12 Lu1 N3 128.0(2) . .
N1 Lu1 N3 122.2(2) . .
Lu1 Lu1 N3 119.94(10) 2_567 .
N1 Lu1 N3 157.87(17) 2_667 .
O4 Lu1 N1 113.00(17) . 2_567
O7 Lu1 N1 112.0(2) . 2_567
O2 Lu1 N1 49.31(17) 2_567 2_567
O2 Lu1 N1 47.61(18) . 2_567
O23 Lu1 N1 51.5(2) . 2_567
O11 Lu1 N1 155.3(2) . 2_567
O12 Lu1 N1 113.9(2) . 2_567
N1 Lu1 N1 137.95(15) . 2_567
Lu1 Lu1 N1 32.61(12) 2_567 2_567
N1 Lu1 N1 109.13(19) 2_667 2_567
N3 Lu1 N1 92.79(14) . 2_567
O3 Lu2 O8 141.03(18) 2_577 1_565
O3 Lu2 O3 72.40(19) 2_577 .
O8 Lu2 O3 143.34(16) 1_565 .
O3 Lu2 O7 85.07(17) 2_577 1_565
O8 Lu2 O7 60.09(17) 1_565 1_565
O3 Lu2 O7 156.54(16) . 1_565
O3 Lu2 O24 81.0(2) 2_577 .
O8 Lu2 O24 83.4(2) 1_565 .
O3 Lu2 O24 90.6(2) . .
O7 Lu2 O24 92.2(2) 1_565 .
O3 Lu2 O15 126.5(2) 2_577 .
O8 Lu2 O15 80.6(2) 1_565 .
O3 Lu2 O15 87.2(2) . .
O7 Lu2 O15 101.6(2) 1_565 .
O24 Lu2 O15 149.8(2) . .
O3 Lu2 O14 77.1(2) 2_577 .
O8 Lu2 O14 110.8(2) 1_565 .
O3 Lu2 O14 87.6(3) . .
O7 Lu2 O14 80.9(3) 1_565 .
O24 Lu2 O14 157.5(2) . .
O15 Lu2 O14 52.5(3) . .
O3 Lu2 O1 126.06(16) 2_577 .
O8 Lu2 O1 85.61(16) 1_565 .
O3 Lu2 O1 57.74(15) . .
O7 Lu2 O1 145.60(15) 1_565 .
O24 Lu2 O1 80.4(2) . .
O15 Lu2 O1 73.1(2) . .
O14 Lu2 O1 117.0(2) . .
O3 Lu2 B3 113.30(19) 2_577 1_565
O8 Lu2 B3 30.08(19) 1_565 1_565
O3 Lu2 B3 173.26(19) . 1_565
O7 Lu2 B3 30.02(19) 1_565 1_565
O24 Lu2 B3 86.8(2) . 1_565
O15 Lu2 B3 91.8(3) . 1_565
O14 Lu2 B3 97.1(3) . 1_565
O1 Lu2 B3 115.62(19) . 1_565
O3 Lu2 N2 102.1(2) 2_577 .
O8 Lu2 N2 95.9(2) 1_565 .
O3 Lu2 N2 87.3(2) . .
O7 Lu2 N2 91.2(2) 1_565 .
O24 Lu2 N2 175.6(3) . .
O15 Lu2 N2 26.1(3) . .
O14 Lu2 N2 26.4(3) . .
O1 Lu2 N2 95.2(2) . .
B3 Lu2 N2 94.7(2) 1_565 .
O3 Lu2 B1 98.79(18) 2_577 .
O8 Lu2 B1 115.51(18) 1_565 .
O3 Lu2 B1 27.84(17) . .
O7 Lu2 B1 175.49(18) 1_565 .
O24 Lu2 B1 86.1(2) . .
O15 Lu2 B1 78.1(3) . .
O14 Lu2 B1 102.2(3) . .
O1 Lu2 B1 29.94(17) . .
B3 Lu2 B1 145.5(2) 1_565 .
N2 Lu2 B1 90.2(2) . .
O3 Lu2 Lu2 36.90(12) 2_577 2_577
O8 Lu2 Lu2 168.22(15) 1_565 2_577
O3 Lu2 Lu2 35.50(11) . 2_577
O7 Lu2 Lu2 121.70(12) 1_565 2_577
O24 Lu2 Lu2 84.91(16) . 2_577
O15 Lu2 Lu2 109.34(19) . 2_577
O14 Lu2 Lu2 80.7(2) . 2_577
O1 Lu2 Lu2 91.28(10) . 2_577
B3 Lu2 Lu2 150.06(15) 1_565 2_577
N2 Lu2 Lu2 95.66(15) . 2_577
B1 Lu2 Lu2 62.36(13) . 2_577
O9 Lu3 O4 146.01(17) 2_566 .
O9 Lu3 O9 73.13(19) 2_566 .
O4 Lu3 O9 138.74(17) . .
O9 Lu3 O25 93.9(2) 2_566 .
O4 Lu3 O25 83.0(2) . .
O9 Lu3 O25 81.2(2) . .
O9 Lu3 O5 85.80(16) 2_566 .
O4 Lu3 O5 60.22(17) . .
O9 Lu3 O5 152.25(17) . .
O25 Lu3 O5 82.4(2) . .
O9 Lu3 O18 89.4(3) 2_566 .
O4 Lu3 O18 107.4(3) . .
O9 Lu3 O18 76.4(2) . .
O25 Lu3 O18 155.4(2) . .
O5 Lu3 O18 122.1(2) . .
O9 Lu3 O17 92.9(3) 2_566 .
O4 Lu3 O17 76.6(3) . .
O9 Lu3 O17 126.3(2) . .
O25 Lu3 O17 152.4(2) . .
O5 Lu3 O17 71.4(2) . .
O18 Lu3 O17 51.2(3) . .
O9 Lu3 O6 130.62(15) 2_566 .
O4 Lu3 O6 82.82(16) . .
O9 Lu3 O6 57.68(15) . .
O25 Lu3 O6 83.4(2) . .
O5 Lu3 O6 141.66(16) . .
O18 Lu3 O6 76.1(2) . .
O17 Lu3 O6 111.8(3) . .
O9 Lu3 B2 116.0(2) 2_566 .
O4 Lu3 B2 30.10(19) . .
O9 Lu3 B2 163.8(2) . .
O25 Lu3 B2 84.7(2) . .
O5 Lu3 B2 30.40(19) . .
O18 Lu3 B2 115.7(3) . .
O17 Lu3 B2 68.4(3) . .
O6 Lu3 B2 112.83(19) . .
O9 Lu3 B4 100.69(18) 2_566 .
O4 Lu3 B4 112.34(18) . .
O9 Lu3 B4 27.78(17) . .
O25 Lu3 B4 82.6(2) . .
O5 Lu3 B4 164.0(2) . .
O18 Lu3 B4 72.9(2) . .
O17 Lu3 B4 122.3(3) . .
O6 Lu3 B4 29.95(17) . .
B2 Lu3 B4 141.8(2) . .
O9 Lu3 N3 91.5(2) 2_566 .
O4 Lu3 N3 91.9(2) . .
O9 Lu3 N3 101.5(2) . .
O25 Lu3 N3 174.5(2) . .
O5 Lu3 N3 96.8(2) . .
O18 Lu3 N3 25.6(2) . .
O17 Lu3 N3 25.6(2) . .
O6 Lu3 N3 94.0(2) . .
B2 Lu3 N3 91.9(2) . .
B4 Lu3 N3 97.6(2) . .
O9 Lu3 Lu3 37.27(12) 2_566 2_566
O4 Lu3 Lu3 169.50(15) . 2_566
O9 Lu3 Lu3 35.86(11) . 2_566
O25 Lu3 Lu3 86.84(16) . 2_566
O5 Lu3 Lu3 121.01(11) . 2_566
O18 Lu3 Lu3 81.1(2) . 2_566
O17 Lu3 Lu3 113.9(2) . 2_566
O6 Lu3 Lu3 93.45(10) . 2_566
B2 Lu3 Lu3 151.12(16) . 2_566
B4 Lu3 Lu3 63.50(13) . 2_566
N3 Lu3 Lu3 98.17(16) . 2_566
O5 Lu4 O8 95.34(18) . 1_565
O5 Lu4 O10 172.5(2) . 1_565
O8 Lu4 O10 82.31(18) 1_565 1_565
O5 Lu4 O10 102.82(17) . 2_566
O8 Lu4 O10 149.6(2) 1_565 2_566
O10 Lu4 O10 76.50(19) 1_565 2_566
O5 Lu4 O26 87.3(2) . .
O8 Lu4 O26 79.4(2) 1_565 .
O10 Lu4 O26 85.2(2) 1_565 .
O10 Lu4 O26 77.3(2) 2_566 .
O5 Lu4 O21 84.8(3) . .
O8 Lu4 O21 128.3(3) 1_565 .
O10 Lu4 O21 102.3(3) 1_565 .
O10 Lu4 O21 78.1(2) 2_566 .
O26 Lu4 O21 151.8(2) . .
O5 Lu4 O20 98.2(3) . .
O8 Lu4 O20 76.2(3) 1_565 .
O10 Lu4 O20 88.3(3) 1_565 .
O10 Lu4 O20 124.0(3) 2_566 .
O26 Lu4 O20 155.4(3) . .
O21 Lu4 O20 52.8(3) . .
O5 Lu4 N4 91.5(2) . .
O8 Lu4 N4 102.5(3) 1_565 .
O10 Lu4 N4 96.0(2) 1_565 .
O10 Lu4 N4 101.2(2) 2_566 .
O26 Lu4 N4 177.9(2) . .
O21 Lu4 N4 26.2(3) . .
O20 Lu4 N4 26.7(3) . .
O5 Lu4 Lu4 140.46(12) . 2_576
O8 Lu4 Lu4 117.75(14) 1_565 2_576
O10 Lu4 Lu4 38.37(12) 1_565 2_576
O10 Lu4 Lu4 38.13(12) 2_566 2_576
O26 Lu4 Lu4 78.86(17) . 2_576
O21 Lu4 Lu4 90.18(19) . 2_576
O20 Lu4 Lu4 109.8(2) . 2_576
N4 Lu4 Lu4 100.95(17) . 2_576
O5 Lu4 N2 57.36(17) . 1_655
O8 Lu4 N2 88.08(18) 1_565 1_655
O10 Lu4 N2 129.45(18) 1_565 1_655
O10 Lu4 N2 122.25(17) 2_566 1_655
O26 Lu4 N2 141.34(19) . 1_655
O21 Lu4 N2 49.1(2) . 1_655
O20 Lu4 N2 41.4(2) . 1_655
N4 Lu4 N2 38.35(19) . 1_655
Lu4 Lu4 N2 138.09(9) 2_576 1_655
O5 Lu4 N4 122.30(17) . 2_576
O8 Lu4 N4 101.92(19) 1_565 2_576
O10 Lu4 N4 51.74(17) 1_565 2_576
O10 Lu4 N4 47.70(18) 2_566 2_576
O26 Lu4 N4 44.26(19) . 2_576
O21 Lu4 N4 121.5(2) . 2_576
O20 Lu4 N4 139.3(2) . 2_576
N4 Lu4 N4 135.58(12) . 2_576
Lu4 Lu4 N4 34.63(10) 2_576 2_576
N2 Lu4 N4 169.87(16) 1_655 2_576
O5 Lu4 N3 43.56(16) . .
O8 Lu4 N3 105.35(18) 1_565 .
O10 Lu4 N3 130.13(17) 1_565 .
O10 Lu4 N3 73.60(16) 2_566 .
O26 Lu4 N3 49.95(18) . .
O21 Lu4 N3 109.3(2) . .
O20 Lu4 N3 141.6(2) . .
N4 Lu4 N3 128.26(19) . .
Lu4 Lu4 N3 103.24(9) 2_576 .
N2 Lu4 N3 100.30(13) 1_655 .
N4 Lu4 N3 78.75(13) 2_576 .
O2 B1 O3 125.7(6) . .
O2 B1 O1 122.9(6) . .
O3 B1 O1 111.4(6) . .
O2 B1 Lu2 176.3(6) . .
O3 B1 Lu2 51.9(3) . .
O1 B1 Lu2 59.6(3) . .
O2 B1 N2 132.2(5) . .
O3 B1 N2 60.0(4) . .
O1 B1 N2 75.2(4) . .
Lu2 B1 N2 44.59(16) . .
O2 B1 N1 81.0(5) . 1_455
O3 B1 N1 83.6(5) . 1_455
O1 B1 N1 107.1(5) . 1_455
Lu2 B1 N1 95.6(2) . 1_455
N2 B1 N1 51.4(2) . 1_455
O2 B1 N1 57.2(4) . .
O3 B1 N1 139.1(5) . .
O1 B1 N1 80.9(4) . .
Lu2 B1 N1 126.6(3) . .
N2 B1 N1 154.7(2) . .
N1 B1 N1 131.7(3) 1_455 .
O2 B1 N1 50.4(4) . 2_567
O3 B1 N1 86.1(4) . 2_567
O1 B1 N1 143.2(5) . 2_567
Lu2 B1 N1 125.8(3) . 2_567
N2 B1 N1 87.6(2) . 2_567
N1 B1 N1 40.7(2) 1_455 2_567
N1 B1 N1 107.5(2) . 2_567
O2 B1 N2 105.2(4) . 2_577
O3 B1 N2 50.8(4) . 2_577
O1 B1 N2 110.7(4) . 2_577
Lu2 B1 N2 75.54(18) . 2_577
N2 B1 N2 107.56(19) . 2_577
N1 B1 N2 128.5(3) 1_455 2_577
N1 B1 N2 88.3(2) . 2_577
N1 B1 N2 105.4(2) 2_567 2_577
O2 B1 N2 100.2(4) . 1_655
O3 B1 N2 112.2(5) . 1_655
O1 B1 N2 53.6(4) . 1_655
Lu2 B1 N2 83.5(2) . 1_655
N2 B1 N2 122.1(2) . 1_655
N1 B1 N2 157.9(2) 1_455 1_655
N1 B1 N2 43.16(17) . 1_655
N1 B1 N2 149.9(2) 2_567 1_655
N2 B1 N2 72.8(2) 2_577 1_655
O4 B2 O5 115.7(6) . .
O4 B2 O1 123.7(6) . .
O5 B2 O1 120.5(6) . .
O4 B2 Lu3 56.9(3) . .
O5 B2 Lu3 59.6(3) . .
O1 B2 Lu3 169.3(6) . .
O4 B2 N3 68.0(4) . .
O5 B2 N3 75.9(4) . .
O1 B2 N3 123.5(5) . .
Lu3 B2 N3 45.88(17) . .
O4 B2 N2 98.3(5) . 1_655
O5 B2 N2 83.6(4) . 1_655
O1 B2 N2 90.1(4) . 1_655
Lu3 B2 N2 100.4(3) . 1_655
N3 B2 N2 146.2(3) . 1_655
O4 B2 N1 51.3(4) . .
O5 B2 N1 120.0(5) . .
O1 B2 N1 99.5(4) . .
Lu3 B2 N1 88.7(2) . .
N3 B2 N1 118.6(3) . .
N2 B2 N1 51.3(2) 1_655 .
O4 B2 N4 123.8(5) . .
O5 B2 N4 42.6(4) . .
O1 B2 N4 99.9(4) . .
Lu3 B2 N4 86.7(2) . .
N3 B2 N4 117.8(2) . .
N2 B2 N4 43.40(17) 1_655 .
N1 B2 N4 91.5(2) . .
O4 B2 N2 128.1(5) . .
O5 B2 N2 96.9(4) . .
O1 B2 N2 43.4(4) . .
Lu3 B2 N2 126.5(3) . .
N3 B2 N2 83.9(2) . .
N2 B2 N2 125.7(3) 1_655 .
N1 B2 N2 139.7(2) . .
N4 B2 N2 107.7(2) . .
O4 B2 N1 88.1(4) . 1_455
O5 B2 N1 125.3(5) . 1_455
O1 B2 N1 57.8(4) . 1_455
Lu3 B2 N1 112.6(3) . 1_455
N3 B2 N1 68.8(2) . 1_455
N2 B2 N1 143.9(2) 1_655 1_455
N1 B2 N1 113.4(2) . 1_455
N4 B2 N1 148.0(2) . 1_455
N2 B2 N1 40.36(16) . 1_455
O7 B3 O8 115.1(6) . .
O7 B3 O6 120.7(6) . .
O8 B3 O6 124.2(6) . .
O7 B3 Lu2 57.9(3) . 1_545
O8 B3 Lu2 57.2(3) . 1_545
O6 B3 Lu2 178.6(5) . 1_545
O7 B3 N4 86.8(5) . 1_445
O8 B3 N4 91.3(5) . 1_445
O6 B3 N4 90.0(4) . 1_445
Lu2 B3 N4 90.0(2) 1_545 1_445
O7 B3 N2 63.7(4) . 1_545
O8 B3 N2 69.3(4) . 1_545
O6 B3 N2 136.1(5) . 1_545
Lu2 B3 N2 43.83(16) 1_545 1_545
N4 B3 N2 46.21(18) 1_445 1_545
O7 B3 N1 60.6(4) . .
O8 B3 N1 124.9(5) . .
O6 B3 N1 85.8(4) . .
Lu2 B3 N1 93.2(2) 1_545 .
N4 B3 N1 138.2(3) 1_445 .
N2 B3 N1 122.7(2) 1_545 .
O7 B3 N4 132.8(5) . 1_545
O8 B3 N4 50.0(4) . 1_545
O6 B3 N4 90.4(4) . 1_545
Lu2 B3 N4 90.6(2) 1_545 1_545
N4 B3 N4 131.1(3) 1_445 1_545
N2 B3 N4 118.7(2) 1_545 1_545
N1 B3 N4 90.6(2) . 1_545
O7 B3 N3 88.2(4) . .
O8 B3 N3 134.7(5) . .
O6 B3 N3 49.0(4) . .
Lu2 B3 N3 130.3(3) 1_545 .
N4 B3 N3 49.63(18) 1_445 .
N2 B3 N3 90.5(2) 1_545 .
N1 B3 N3 100.3(2) . .
N4 B3 N3 136.2(2) 1_545 .
O10 B4 O9 125.1(6) . .
O10 B4 O6 122.5(6) . .
O9 B4 O6 112.3(5) . .
O10 B4 Lu3 174.4(5) . .
O9 B4 Lu3 51.6(3) . .
O6 B4 Lu3 60.9(3) . .
O10 B4 N3 87.3(4) . 1_655
O9 B4 N3 82.6(4) . 1_655
O6 B4 N3 101.5(4) . 1_655
Lu3 B4 N3 96.4(2) . 1_655
O10 B4 N3 134.5(5) . .
O9 B4 N3 68.0(4) . .
O6 B4 N3 65.4(4) . .
Lu3 B4 N3 41.30(14) . .
N3 B4 N3 137.5(3) 1_655 .
O10 B4 N4 57.4(4) . 2_566
O9 B4 N4 91.8(4) . 2_566
O6 B4 N4 124.5(5) . 2_566
Lu3 B4 N4 117.1(2) . 2_566
N3 B4 N4 131.8(2) 1_655 2_566
N3 B4 N4 80.9(2) . 2_566
O10 B4 N4 48.7(4) . 1_545
O9 B4 N4 130.1(5) . 1_545
O6 B4 N4 95.3(4) . 1_545
Lu3 B4 N4 136.8(3) . 1_545
N3 B4 N4 50.57(18) 1_655 1_545
N3 B4 N4 159.2(2) . 1_545
N4 B4 N4 106.08(19) 2_566 1_545
O10 B4 N3 101.0(4) . 2_566
O9 B4 N3 41.0(4) . 2_566
O6 B4 N3 124.8(4) . 2_566
Lu3 B4 N3 79.02(19) . 2_566
N3 B4 N3 44.5(2) 1_655 2_566
N3 B4 N3 108.10(19) . 2_566
N4 B4 N3 106.49(19) 2_566 2_566
N4 B4 N3 89.06(19) 1_545 2_566
O10 B4 N4 92.8(4) . 1_445
O9 B4 N4 112.6(4) . 1_445
O6 B4 N4 62.3(4) . 1_445
Lu3 B4 N4 85.1(2) . 1_445
N3 B4 N4 160.5(2) 1_655 1_445
N3 B4 N4 48.26(17) . 1_445
N4 B4 N4 62.3(2) 2_566 1_445
N4 B4 N4 117.0(2) 1_545 1_445
N3 B4 N4 153.2(2) 2_566 1_445
O13 N1 O12 122.5(13) . .
O13 N1 O11 122.2(13) . .
O12 N1 O11 115.2(9) . .
O13 N1 Lu1 177.8(10) . .
O12 N1 Lu1 58.6(5) . .
O11 N1 Lu1 56.8(5) . .
O13 N1 O13 101.0(8) . 2_667
O12 N1 O13 82.0(7) . 2_667
O11 N1 O13 83.9(7) . 2_667
Lu1 N1 O13 80.9(3) . 2_667
O13 N1 N1 78.5(8) . 2_667
O12 N1 N1 94.1(7) . 2_667
O11 N1 N1 95.8(7) . 2_667
Lu1 N1 N1 103.4(4) . 2_667
O13 N1 N1 22.5(3) 2_667 2_667
O13 N1 O16 85.1(8) . 1_655
O12 N1 O16 69.6(6) . 1_655
O11 N1 O16 118.4(7) . 1_655
Lu1 N1 O16 93.7(3) . 1_655
O13 N1 O16 149.3(5) 2_667 1_655
N1 N1 O16 145.6(6) 2_667 1_655
O13 N1 O12 67.7(7) . 2_667
O12 N1 O12 115.8(6) . 2_667
O11 N1 O12 86.2(6) . 2_667
Lu1 N1 O12 113.7(3) . 2_667
O13 N1 O12 38.5(3) 2_667 2_667
N1 N1 O12 21.7(3) 2_667 2_667
O16 N1 O12 150.9(4) 1_655 2_667
O13 N1 O4 139.6(8) . .
O12 N1 O4 66.2(5) . .
O11 N1 O4 67.4(5) . .
Lu1 N1 O4 38.55(14) . .
O13 N1 O4 119.3(4) 2_667 .
N1 N1 O4 141.8(5) 2_667 .
O16 N1 O4 59.8(2) 1_655 .
O12 N1 O4 149.3(3) 2_667 .
O13 N1 O11 68.0(8) . 2_667
O12 N1 O11 84.6(6) . 2_667
O11 N1 O11 117.3(6) . 2_667
Lu1 N1 O11 114.1(3) . 2_667
O13 N1 O11 38.2(3) 2_667 2_667
N1 N1 O11 21.5(3) 2_667 2_667
O16 N1 O11 124.2(4) 1_655 2_667
O12 N1 O11 36.4(2) 2_667 2_667
O4 N1 O11 147.6(4) . 2_667
O16 N2 O15 122.0(10) . .
O16 N2 O14 123.0(10) . .
O15 N2 O14 114.9(7) . .
O16 N2 Lu2 178.1(7) . .
O15 N2 Lu2 57.0(4) . .
O14 N2 Lu2 58.0(4) . .
O16 N2 O22 93.1(6) . 1_455
O15 N2 O22 79.1(5) . 1_455
O14 N2 O22 96.4(6) . 1_455
Lu2 N2 O22 85.1(3) . 1_455
O16 N2 N4 70.6(6) . 1_455
O15 N2 N4 92.8(5) . 1_455
O14 N2 N4 106.8(6) . 1_455
Lu2 N2 N4 107.6(3) . 1_455
O22 N2 N4 22.5(2) 1_455 1_455
O16 N2 O13 90.5(7) . 1_455
O15 N2 O13 70.7(6) . 1_455
O14 N2 O13 109.5(6) . 1_455
Lu2 N2 O13 90.6(3) . 1_455
O22 N2 O13 146.3(5) 1_455 1_455
N4 N2 O13 143.7(4) 1_455 1_455
O16 N2 O20 61.8(6) . 1_455
O15 N2 O20 114.5(5) . 1_455
O14 N2 O20 94.6(6) . 1_455
Lu2 N2 O20 116.8(3) . 1_455
O22 N2 O20 38.6(3) 1_455 1_455
N4 N2 O20 21.7(2) 1_455 1_455
O13 N2 O20 150.7(4) 1_455 1_455
O16 N2 N1 71.0(6) . 1_455
O15 N2 N1 84.9(6) . 1_455
O14 N2 N1 116.9(6) . 1_455
Lu2 N2 N1 110.2(3) . 1_455
O22 N2 N1 146.7(4) 1_455 1_455
N4 N2 N1 132.8(4) 1_455 1_455
O13 N2 N1 19.8(2) 1_455 1_455
O20 N2 N1 132.4(3) 1_455 1_455
O16 N2 O12 61.1(6) . 1_455
O15 N2 O12 105.5(6) . 1_455
O14 N2 O12 105.6(6) . 1_455
Lu2 N2 O12 120.6(3) . 1_455
O22 N2 O12 152.4(3) 1_455 1_455
N4 N2 O12 131.1(3) 1_455 1_455
O13 N2 O12 37.0(3) 1_455 1_455
O20 N2 O12 121.4(3) 1_455 1_455
N1 N2 O12 20.7(2) 1_455 1_455
O19 N3 O17 122.7(9) . .
O19 N3 O18 122.0(9) . .
O17 N3 O18 115.1(8) . .
O19 N3 Lu3 175.7(7) . .
O17 N3 Lu3 59.1(5) . .
O18 N3 Lu3 56.0(5) . .
O19 N3 O19 87.8(6) . 2_466
O17 N3 O19 81.6(6) . 2_466
O18 N3 O19 95.7(6) . 2_466
Lu3 N3 O19 88.6(3) . 2_466
O19 N3 N3 66.3(6) . 2_466
O17 N3 N3 93.8(7) . 2_466
O18 N3 N3 106.6(7) . 2_466
Lu3 N3 N3 110.1(3) . 2_466
O19 N3 N3 21.57(19) 2_466 2_466
O19 N3 O25 53.1(6) . 1_455
O17 N3 O25 69.6(5) . 1_455
O18 N3 O25 174.1(6) . 1_455
Lu3 N3 O25 128.7(3) . 1_455
O19 N3 O25 81.3(3) 2_466 1_455
N3 N3 O25 68.9(3) 2_466 1_455
O19 N3 O26 51.6(6) . 2_466
O17 N3 O26 165.4(7) . 2_466
O18 N3 O26 71.0(5) . 2_466
Lu3 N3 O26 125.5(3) . 2_466
O19 N3 O26 84.6(3) 2_466 2_466
N3 N3 O26 71.7(3) 2_466 2_466
O25 N3 O26 103.5(2) 1_455 2_466
O19 N3 O20 63.4(6) . 1_445
O17 N3 O20 125.2(7) . 1_445
O18 N3 O20 88.4(6) . 1_445
Lu3 N3 O20 119.3(3) . 1_445
O19 N3 O20 147.8(3) 2_466 1_445
N3 N3 O20 127.6(4) 2_466 1_445
O25 N3 O20 91.5(2) 1_455 1_445
O26 N3 O20 66.5(2) 2_466 1_445
O19 N3 O17 56.3(6) . 2_466
O17 N3 O17 113.8(6) . 2_466
O18 N3 O17 96.7(6) . 2_466
Lu3 N3 O17 119.5(3) . 2_466
O19 N3 O17 36.6(2) 2_466 2_466
N3 N3 O17 20.0(2) 2_466 2_466
O25 N3 O17 77.8(2) 1_455 2_466
O26 N3 O17 51.7(2) 2_466 2_466
O20 N3 O17 111.3(3) 1_445 2_466
O22 N4 O21 122.9(11) . .
O22 N4 O20 121.2(10) . .
O21 N4 O20 115.8(8) . .
O22 N4 Lu4 177.6(7) . .
O21 N4 Lu4 57.6(5) . .
O20 N4 Lu4 58.2(5) . .
O22 N4 O16 91.9(7) . 1_655
O21 N4 O16 94.8(6) . 1_655
O20 N4 O16 80.7(6) . 1_655
Lu4 N4 O16 85.6(3) . 1_655
O22 N4 N2 69.5(6) . 1_655
O21 N4 N2 108.2(6) . 1_655
O20 N4 N2 91.2(6) . 1_655
Lu4 N4 N2 108.1(3) . 1_655
O16 N4 N2 22.5(2) 1_655 1_655
O22 N4 O18 63.3(6) . 1_665
O21 N4 O18 114.5(6) . 1_665
O20 N4 O18 95.4(6) . 1_665
Lu4 N4 O18 118.9(3) . 1_665
O16 N4 O18 148.6(4) 1_655 1_665
N2 N4 O18 128.2(3) 1_655 1_665
O22 N4 O15 57.7(6) . 1_655
O21 N4 O15 99.1(6) . 1_655
O20 N4 O15 112.3(6) . 1_655
Lu4 N4 O15 120.1(3) . 1_655
O16 N4 O15 38.2(2) 1_655 1_655
N2 N4 O15 21.1(2) 1_655 1_655
O18 N4 O15 120.9(3) 1_665 1_655
O22 N4 O19 95.8(7) . 1_665
O21 N4 O19 110.1(6) . 1_665
O20 N4 O19 65.0(6) . 1_665
Lu4 N4 O19 86.1(2) . 1_665
O16 N4 O19 143.7(4) 1_655 1_665
N2 N4 O19 140.9(4) 1_655 1_665
O18 N4 O19 35.71(19) 1_665 1_665
O15 N4 O19 148.7(3) 1_655 1_665
O22 N4 O5 141.3(7) . .
O21 N4 O5 55.9(5) . .
O20 N4 O5 73.1(5) . .
Lu4 N4 O5 36.57(13) . .
O16 N4 O5 52.7(2) 1_655 .
N2 N4 O5 74.8(2) 1_655 .
O18 N4 O5 155.4(3) 1_665 .
O15 N4 O5 83.7(2) 1_655 .
O19 N4 O5 121.8(3) 1_665 .
B2 O1 B1 128.2(5) . .
B2 O1 Lu2 140.8(4) . .
B1 O1 Lu2 90.5(4) . .
B2 O1 N2 122.4(4) . .
B1 O1 N2 84.2(4) . .
Lu2 O1 N2 46.00(15) . .
B2 O1 N2 70.8(4) . 1_655
B1 O1 N2 110.9(4) . 1_655
Lu2 O1 N2 104.39(19) . 1_655
N2 O1 N2 148.3(3) . 1_655
B2 O1 N1 62.8(4) . .
B1 O1 N1 81.1(4) . .
Lu2 O1 N1 141.8(2) . .
N2 O1 N1 163.1(2) . .
N2 O1 N1 46.95(17) 1_655 .
B2 O1 N1 107.6(5) . 1_455
B1 O1 N1 56.2(4) . 1_455
Lu2 O1 N1 87.37(19) . 1_455
N2 O1 N1 47.04(18) . 1_455
N2 O1 N1 163.17(18) 1_655 1_455
N1 O1 N1 116.8(2) . 1_455
B2 O1 N3 42.8(4) . .
B1 O1 N3 112.6(4) . .
Lu2 O1 N3 122.68(19) . .
N2 O1 N3 83.44(18) . .
N2 O1 N3 113.47(18) 1_655 .
N1 O1 N3 94.70(19) . .
N1 O1 N3 67.82(18) 1_455 .
B2 O1 N4 63.8(4) . .
B1 O1 N4 147.8(5) . .
Lu2 O1 N4 87.36(16) . .
N2 O1 N4 115.89(18) . .
N2 O1 N4 39.68(14) 1_655 .
N1 O1 N4 80.95(17) . .
N1 O1 N4 155.45(19) 1_455 .
N3 O1 N4 95.29(16) . .
B1 O2 Lu1 126.2(4) . 2_567
B1 O2 Lu1 129.1(4) . .
Lu1 O2 Lu1 103.84(19) 2_567 .
B1 O2 N1 114.2(5) . 2_567
Lu1 O2 N1 45.13(17) 2_567 2_567
Lu1 O2 N1 107.4(2) . 2_567
B1 O2 N1 106.3(5) . .
Lu1 O2 N1 105.7(2) 2_567 .
Lu1 O2 N1 43.73(19) . .
N1 O2 N1 139.22(16) 2_567 .
B1 O2 N1 80.1(5) . 1_455
Lu1 O2 N1 88.7(2) 2_567 1_455
Lu1 O2 N1 113.0(2) . 1_455
N1 O2 N1 45.0(2) 2_567 1_455
N1 O2 N1 154.5(3) . 1_455
B1 O2 N2 36.3(4) . .
Lu1 O2 N2 115.97(18) 2_567 .
Lu1 O2 N2 130.08(19) . .
N1 O2 N2 83.35(18) 2_567 .
N1 O2 N2 136.07(19) . .
N1 O2 N2 43.94(17) 1_455 .
B1 O3 Lu2 146.3(4) . 2_577
B1 O3 Lu2 100.3(4) . .
Lu2 O3 Lu2 107.60(19) 2_577 .
B1 O3 N2 100.7(4) . .
Lu2 O3 N2 111.2(2) 2_577 .
Lu2 O3 N2 52.70(16) . .
B1 O3 N2 113.8(5) . 2_577
Lu2 O3 N2 44.60(16) 2_577 2_577
Lu2 O3 N2 97.81(19) . 2_577
N2 O3 N2 138.88(15) . 2_577
B1 O3 N1 77.6(4) . 1_455
Lu2 O3 N1 112.5(2) 2_577 1_455
Lu2 O3 N1 104.1(2) . 1_455
N2 O3 N1 53.56(19) . 1_455
N2 O3 N1 153.1(2) 2_577 1_455
B1 O3 N1 77.3(4) . 2_567
Lu2 O3 N1 90.53(19) 2_577 2_567
Lu2 O3 N1 143.8(2) . 2_567
N2 O3 N1 91.8(2) . 2_567
N2 O3 N1 116.41(19) 2_577 2_567
N1 O3 N1 39.8(2) 1_455 2_567
B2 O4 Lu1 131.4(4) . .
B2 O4 Lu3 93.0(4) . .
Lu1 O4 Lu3 135.7(2) . .
B2 O4 N1 110.7(5) . .
Lu1 O4 N1 55.45(19) . .
Lu3 O4 N1 115.8(3) . .
B2 O4 N3 92.3(4) . .
Lu1 O4 N3 116.1(2) . .
Lu3 O4 N3 50.70(17) . .
N1 O4 N3 154.9(3) . .
B2 O4 N2 64.2(4) . 1_655
Lu1 O4 N2 102.3(2) . 1_655
Lu3 O4 N2 97.63(19) . 1_655
N1 O4 N2 51.2(2) . 1_655
N3 O4 N2 141.2(2) . 1_655
B2 O5 Lu4 141.6(4) . .
B2 O5 Lu3 90.0(4) . .
Lu4 O5 Lu3 127.6(2) . .
B2 O5 N4 122.6(5) . .
Lu4 O5 N4 51.91(17) . .
Lu3 O5 N4 117.1(2) . .
B2 O5 N3 84.3(4) . .
Lu4 O5 N3 114.1(2) . .
Lu3 O5 N3 47.03(15) . .
N4 O5 N3 151.4(2) . .
B2 O5 N2 77.3(4) . 1_655
Lu4 O5 N2 96.7(2) . 1_655
Lu3 O5 N2 105.7(2) . 1_655
N4 O5 N2 47.98(18) . 1_655
N3 O5 N2 147.3(2) . 1_655
B2 O5 N1 46.2(4) . .
Lu4 O5 N1 141.6(2) . .
Lu3 O5 N1 74.57(18) . .
N4 O5 N1 91.0(2) . .
N3 O5 N1 103.65(19) . .
N2 O5 N1 44.84(17) 1_655 .
B2 O5 N2 67.9(4) . .
Lu4 O5 N2 81.76(16) . .
Lu3 O5 N2 125.4(2) . .
N4 O5 N2 116.9(2) . .
N3 O5 N2 80.37(18) . .
N2 O5 N2 116.1(2) 1_655 .
N1 O5 N2 112.32(17) . .
B3 O6 B4 127.3(5) . .
B3 O6 Lu3 143.2(4) . .
B4 O6 Lu3 89.1(4) . .
B3 O6 N3 115.3(4) . .
B4 O6 N3 95.4(4) . .
Lu3 O6 N3 46.68(14) . .
B3 O6 N4 70.6(4) . 1_445
B4 O6 N4 100.5(4) . 1_445
Lu3 O6 N4 100.40(18) . 1_445
N3 O6 N4 53.76(17) . 1_445
B3 O6 N1 75.8(4) . .
B4 O6 N1 132.5(4) . .
Lu3 O6 N1 83.06(17) . .
N3 O6 N1 111.7(2) . .
N4 O6 N1 127.0(2) 1_445 .
B3 O6 N3 110.7(4) . 1_655
B4 O6 N3 61.1(4) . 1_655
Lu3 O6 N3 90.46(16) . 1_655
N3 O6 N3 133.3(2) . 1_655
N4 O6 N3 158.7(2) 1_445 1_655
N1 O6 N3 72.15(18) . 1_655
B3 O6 N4 72.7(4) . 1_545
B4 O6 N4 67.7(4) . 1_545
Lu3 O6 N4 136.16(19) . 1_545
N3 O6 N4 161.35(19) . 1_545
N4 O6 N4 119.5(2) 1_445 1_545
N1 O6 N4 86.35(19) . 1_545
N3 O6 N4 45.95(15) 1_655 1_545
B3 O7 Lu1 132.8(5) . .
B3 O7 Lu2 92.1(4) . 1_545
Lu1 O7 Lu2 129.5(2) . 1_545
B3 O7 N2 97.0(4) . 1_545
Lu1 O7 N2 125.4(2) . 1_545
Lu2 O7 N2 50.27(17) 1_545 1_545
B3 O7 N1 101.6(5) . .
Lu1 O7 N1 45.9(2) . .
Lu2 O7 N1 114.4(2) 1_545 .
N2 O7 N1 156.5(2) 1_545 .
B3 O7 N4 74.3(5) . 1_445
Lu1 O7 N4 117.8(2) . 1_445
Lu2 O7 N4 92.5(2) 1_545 1_445
N2 O7 N4 47.21(17) 1_545 1_445
N1 O7 N4 153.1(2) . 1_445
B3 O7 N3 75.7(4) . .
Lu1 O7 N3 81.71(17) . .
Lu2 O7 N3 140.2(2) 1_545 .
N2 O7 N3 93.13(19) 1_545 .
N1 O7 N3 105.17(19) . .
N4 O7 N3 47.88(16) 1_445 .
B3 O8 Lu4 131.3(4) . 1_545
B3 O8 Lu2 92.7(4) . 1_545
Lu4 O8 Lu2 135.7(2) 1_545 1_545
B3 O8 N2 91.2(4) . 1_545
Lu4 O8 N2 122.8(2) 1_545 1_545
Lu2 O8 N2 47.62(16) 1_545 1_545
B3 O8 N4 114.6(5) . 1_545
Lu4 O8 N4 44.99(18) 1_545 1_545
Lu2 O8 N4 119.1(2) 1_545 1_545
N2 O8 N4 152.8(2) 1_545 1_545
B3 O8 N4 70.2(4) . 1_445
Lu4 O8 N4 107.5(2) 1_545 1_445
Lu2 O8 N4 90.1(2) 1_545 1_445
N2 O8 N4 45.81(17) 1_545 1_445
N4 O8 N4 149.2(3) 1_545 1_445
B4 O9 Lu3 151.5(4) . 2_566
B4 O9 Lu3 100.7(4) . .
Lu3 O9 Lu3 106.87(18) 2_566 .
B4 O9 N3 124.9(4) . 2_566
Lu3 O9 N3 51.54(16) 2_566 2_566
Lu3 O9 N3 109.3(2) . 2_566
B4 O9 N3 93.7(4) . .
Lu3 O9 N3 100.59(19) 2_566 .
Lu3 O9 N3 44.62(15) . .
N3 O9 N3 139.54(15) 2_566 .
B4 O9 N3 78.7(4) . 1_655
Lu3 O9 N3 100.3(2) 2_566 1_655
Lu3 O9 N3 105.9(2) . 1_655
N3 O9 N3 49.4(2) 2_566 1_655
N3 O9 N3 148.1(2) . 1_655
B4 O9 N4 71.5(4) . 2_566
Lu3 O9 N4 86.39(17) 2_566 2_566
Lu3 O9 N4 125.3(2) . 2_566
N3 O9 N4 119.31(19) 2_566 2_566
N3 O9 N4 81.15(19) . 2_566
N3 O9 N4 124.00(19) 1_655 2_566
B4 O10 Lu4 131.1(4) . 1_545
B4 O10 Lu4 124.6(4) . 2_566
Lu4 O10 Lu4 103.50(19) 1_545 2_566
B4 O10 N4 115.8(4) . 1_545
Lu4 O10 N4 48.30(16) 1_545 1_545
Lu4 O10 N4 106.4(2) 2_566 1_545
B4 O10 N4 105.9(4) . 2_566
Lu4 O10 N4 102.0(2) 1_545 2_566
Lu4 O10 N4 45.02(17) 2_566 2_566
N4 O10 N4 138.21(16) 1_545 2_566
B4 O10 N3 74.6(4) . 1_655
Lu4 O10 N3 101.8(2) 1_545 1_655
Lu4 O10 N3 106.2(2) 2_566 1_655
N4 O10 N3 54.32(18) 1_545 1_655
N4 O10 N3 146.5(2) 2_566 1_655
B4 O10 N4 71.7(4) . 1_445
Lu4 O10 N4 86.59(17) 1_545 1_445
Lu4 O10 N4 108.5(2) 2_566 1_445
N4 O10 N4 128.1(2) 1_545 1_445
N4 O10 N4 63.5(2) 2_566 1_445
N3 O10 N4 141.18(19) 1_655 1_445
B4 O10 N3 63.8(4) . 2_566
Lu4 O10 N3 140.1(2) 1_545 2_566
Lu4 O10 N3 81.15(16) 2_566 2_566
N4 O10 N3 92.10(19) 1_545 2_566
N4 O10 N3 108.08(17) 2_566 2_566
N3 O10 N3 41.01(18) 1_655 2_566
N4 O10 N3 130.15(17) 1_445 2_566
N1 O13 N1 79.0(8) . 2_667
N1 O13 N2 95.0(8) . 1_655
N1 O13 N2 145.7(6) 2_667 1_655
N1 O13 N3 98.6(10) . 1_655
N1 O13 N3 125.9(5) 2_667 1_655
N2 O13 N3 88.3(3) 1_655 1_655
N1 O12 Lu1 94.9(6) . .
N1 O12 N1 64.2(6) . 2_667
Lu1 O12 N1 104.0(3) . 2_667
N1 O12 N2 79.5(6) . 1_655
Lu1 O12 N2 126.3(3) . 1_655
N1 O12 N2 119.9(3) 2_667 1_655
N1 O11 Lu1 96.8(6) . .
N1 O11 N1 62.7(6) . 2_667
Lu1 O11 N1 103.9(3) . 2_667
N1 O11 N2 36.5(5) . 1_655
Lu1 O11 N2 97.8(3) . 1_655
N1 O11 N2 98.0(3) 2_667 1_655
N1 O11 N3 103.4(6) . 1_655
Lu1 O11 N3 136.0(3) . 1_655
N1 O11 N3 120.1(3) 2_667 1_655
N2 O11 N3 77.9(2) 1_655 1_655
N2 O16 N4 86.8(6) . 1_455
N2 O16 N1 88.7(7) . 1_455
N4 O16 N1 151.5(5) 1_455 1_455
N2 O15 Lu2 96.9(5) . .
N2 O15 N4 66.0(5) . 1_455
Lu2 O15 N4 110.3(3) . 1_455
N2 O15 N1 75.0(5) . 1_455
Lu2 O15 N1 118.9(3) . 1_455
N4 O15 N1 119.6(3) 1_455 1_455
N2 O15 N3 137.7(6) . .
Lu2 O15 N3 124.1(3) . .
N4 O15 N3 103.9(2) 1_455 .
N1 O15 N3 76.1(2) 1_455 .
N2 O14 Lu2 95.7(5) . .
N2 O14 N4 54.4(5) . 1_455
Lu2 O14 N4 101.9(3) . 1_455
N2 O14 N1 47.8(5) . 1_455
Lu2 O14 N1 99.7(3) . 1_455
N4 O14 N1 100.3(2) 1_455 1_455
N2 O14 N2 120.6(5) . 2_477
Lu2 O14 N2 134.4(3) . 2_477
N4 O14 N2 121.1(2) 1_455 2_477
N1 O14 N2 87.7(2) 1_455 2_477
N3 O17 Lu3 95.3(6) . .
N3 O17 N3 66.2(6) . 2_466
Lu3 O17 N3 111.6(3) . 2_466
N3 O17 N4 34.1(5) . 1_445
Lu3 O17 N4 90.6(3) . 1_445
N3 O17 N4 99.4(2) 2_466 1_445
N3 O17 N1 105.0(6) . 1_455
Lu3 O17 N1 131.6(3) . 1_455
N3 O17 N1 116.8(3) 2_466 1_455
N4 O17 N1 83.4(2) 1_445 1_455
N3 O17 N2 136.0(6) . .
Lu3 O17 N2 127.8(3) . .
N3 O17 N2 100.0(2) 2_466 .
N4 O17 N2 124.7(3) 1_445 .
N1 O17 N2 41.84(17) 1_455 .
N3 O19 N3 92.2(6) . 2_466
N3 O19 N4 86.2(6) . 1_445
N3 O19 N4 147.2(4) 2_466 1_445
N3 O18 Lu3 98.4(6) . .
N3 O18 N4 91.7(6) . 1_445
Lu3 O18 N4 129.2(4) . 1_445
N3 O18 N3 55.3(6) . 2_466
Lu3 O18 N3 105.8(3) . 2_466
N4 O18 N3 120.4(3) 1_445 2_466
N3 O18 N4 138.6(6) . 2_566
Lu3 O18 N4 122.3(3) . 2_566
N4 O18 N4 69.7(3) 1_445 2_566
N3 O18 N4 101.8(2) 2_466 2_566
N4 O22 N2 88.0(7) . 1_655
N4 O22 N3 84.4(6) . 1_665
N2 O22 N3 141.8(5) 1_655 1_665
N4 O22 N4 86.5(7) . 2_676
N2 O22 N4 131.5(4) 1_655 2_676
N3 O22 N4 85.4(3) 1_665 2_676
N4 O21 Lu4 96.2(6) . .
N4 O21 N2 53.4(5) . 1_655
Lu4 O21 N2 102.0(3) . 1_655
N4 O21 N4 111.7(6) . 2_676
Lu4 O21 N4 133.2(3) . 2_676
N2 O21 N4 124.8(3) 1_655 2_676
N4 O21 N3 45.0(5) . 1_665
Lu4 O21 N3 93.6(3) . 1_665
N2 O21 N3 97.9(2) 1_655 1_665
N4 O21 N3 82.2(2) 2_676 1_665
N4 O21 N3 137.3(6) . 2_566
Lu4 O21 N3 125.0(3) . 2_566
N2 O21 N3 102.3(2) 1_655 2_566
N4 O21 N3 49.05(18) 2_676 2_566
N3 O21 N3 130.23(19) 1_665 2_566
N4 O20 Lu4 95.2(6) . .
N4 O20 N2 67.1(5) . 1_655
Lu4 O20 N2 111.0(3) . 1_655
N4 O20 N3 84.2(6) . 1_665
Lu4 O20 N3 118.7(3) . 1_665
N2 O20 N3 124.1(3) 1_655 1_665
Lu1 O23 N1 123.0(3) . 1_455
Lu1 O23 N3 106.9(3) . .
N1 O23 N3 90.6(2) 1_455 .
Lu1 O23 N4 122.1(3) . 1_445
N1 O23 N4 113.2(3) 1_455 1_445
N3 O23 N4 57.6(2) . 1_445
Lu1 O23 N1 101.4(3) . 2_567
N1 O23 N1 46.4(2) 1_455 2_567
N3 O23 N1 136.9(3) . 2_567
N4 O23 N1 128.4(3) 1_445 2_567
Lu1 O23 N2 102.4(2) . 1_545
N1 O23 N2 126.5(3) 1_455 1_545
N3 O23 N2 102.6(2) . 1_545
N4 O23 N2 46.02(18) 1_445 1_545
N1 O23 N2 102.3(2) 2_567 1_545
Lu1 O23 N1 6.14(14) . .
N1 O23 N1 124.4(3) 1_455 .
N3 O23 N1 100.8(2) . .
N4 O23 N1 118.8(2) 1_445 .
N1 O23 N1 106.7(2) 2_567 .
N2 O23 N1 103.9(2) 1_545 .
Lu2 O24 N2 127.6(3) . 1_655
Lu2 O24 N2 102.8(2) . 2_577
N2 O24 N2 100.1(2) 1_655 2_577
Lu2 O24 N1 118.1(3) . 2_677
N2 O24 N1 113.7(3) 1_655 2_677
N2 O24 N1 54.6(2) 2_577 2_677
Lu2 O24 N4 107.0(2) . .
N2 O24 N4 46.47(18) 1_655 .
N2 O24 N4 144.9(3) 2_577 .
N1 O24 N4 121.9(2) 2_677 .
Lu2 O24 N1 100.0(2) . 1_565
N2 O24 N1 123.7(2) 1_655 1_565
N2 O24 N1 96.1(2) 2_577 1_565
N1 O24 N1 43.4(2) 2_677 1_565
N4 O24 N1 96.5(2) . 1_565
Lu2 O24 N2 2.44(14) . .
N2 O24 N2 125.2(3) 1_655 .
N2 O24 N2 103.22(18) 2_577 .
N1 O24 N2 120.3(2) 2_677 .
N4 O24 N2 105.8(2) . .
N1 O24 N2 102.3(2) 1_565 .
Lu3 O25 N3 127.3(3) . 1_655
Lu3 O25 N2 122.4(3) . 1_655
N3 O25 N2 109.6(3) 1_655 1_655
Lu3 O25 N1 105.2(3) . .
N3 O25 N1 94.8(3) 1_655 .
N2 O25 N1 57.2(2) 1_655 .
Lu3 O25 N3 101.2(2) . 2_566
N3 O25 N3 52.4(2) 1_655 2_566
N2 O25 N3 122.3(2) 1_655 2_566
N1 O25 N3 146.5(3) . 2_566
Lu3 O25 N4 101.7(2) . .
N3 O25 N4 120.4(3) 1_655 .
N2 O25 N4 47.99(19) 1_655 .
N1 O25 N4 103.7(3) . .
N3 O25 N4 90.6(2) 2_566 .
Lu3 O25 N3 3.06(13) . .
N3 O25 N3 128.1(3) 1_655 .
N2 O25 N3 120.9(2) 1_655 .
N1 O25 N3 102.1(2) . .
N3 O25 N3 104.02(18) 2_566 .
N4 O25 N3 102.7(2) . .
Lu4 O26 N3 128.5(3) . 2_466
Lu4 O26 N4 108.9(3) . 2_576
N3 O26 N4 62.1(2) 2_466 2_576
Lu4 O26 N4 125.9(3) . 1_455
N3 O26 N4 104.1(3) 2_466 1_455
N4 O26 N4 82.7(3) 2_576 1_455
Lu4 O26 N3 104.0(2) . .
N3 O26 N3 51.0(2) 2_466 .
N4 O26 N3 112.2(2) 2_576 .
N4 O26 N3 120.4(2) 1_455 .
Lu4 O26 N2 106.1(2) . .
N3 O26 N2 117.5(2) 2_466 .
N4 O26 N2 130.0(2) 2_576 .
N4 O26 N2 47.70(19) 1_455 .
N3 O26 N2 92.2(2) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Lu1 O4 2.137(5) .
Lu1 O7 2.156(5) .
Lu1 O2 2.219(4) 2_567
Lu1 O2 2.241(5) .
Lu1 O23 2.349(7) .
Lu1 O11 2.379(8) .
Lu1 O12 2.420(8) .
Lu1 N1 2.824(9) .
Lu1 Lu1 3.5103(5) 2_567
Lu1 N1 4.631(9) 2_667
Lu1 N3 5.026(8) .
Lu1 N1 5.054(10) 2_567
Lu2 O3 2.209(4) 2_577
Lu2 O8 2.274(5) 1_565
Lu2 O3 2.285(4) .
Lu2 O7 2.290(5) 1_565
Lu2 O24 2.315(7) .
Lu2 O15 2.389(7) .
Lu2 O14 2.409(7) .
Lu2 O1 2.463(5) .
Lu2 B3 2.702(7) 1_565
Lu2 N2 2.828(8) .
Lu2 B1 2.857(7) .
Lu2 Lu2 3.6266(5) 2_577
Lu3 O9 2.203(4) 2_566
Lu3 O4 2.252(5) .
Lu3 O9 2.277(4) .
Lu3 O25 2.292(7) .
Lu3 O5 2.314(5) .
Lu3 O18 2.403(8) .
Lu3 O17 2.473(8) .
Lu3 O6 2.497(4) .
Lu3 B2 2.684(7) .
Lu3 B4 2.857(7) .
Lu3 N3 2.869(8) .
Lu3 Lu3 3.5985(5) 2_566
Lu4 O5 2.143(5) .
Lu4 O8 2.151(5) 1_565
Lu4 O10 2.214(5) 1_565
Lu4 O10 2.226(5) 2_566
Lu4 O26 2.333(6) .
Lu4 O21 2.405(7) .
Lu4 O20 2.415(8) .
Lu4 N4 2.831(8) .
Lu4 Lu4 3.4870(5) 2_576
Lu4 N2 4.869(7) 1_655
Lu4 N4 4.891(8) 2_576
Lu4 N3 5.155(8) .
B1 O2 1.345(8) .
B1 O3 1.356(8) .
B1 O1 1.426(8) .
B1 N2 4.029(11) .
B1 N1 4.105(12) 1_455
B1 N1 4.546(12) .
B1 N1 4.627(12) 2_567
B1 N2 4.653(11) 2_577
B1 N2 4.980(11) 1_655
B2 O4 1.348(9) .
B2 O5 1.358(8) .
B2 O1 1.400(8) .
B2 N3 3.994(11) .
B2 N2 4.052(11) 1_655
B2 N1 4.097(11) .
B2 N4 4.476(12) .
B2 N2 4.813(11) .
B2 N1 5.318(12) 1_455
B3 O7 1.353(8) .
B3 O8 1.356(9) .
B3 O6 1.412(8) .
B3 Lu2 2.702(7) 1_545
B3 N4 4.028(12) 1_445
B3 N2 4.070(11) 1_545
B3 N1 4.341(13) .
B3 N4 4.641(12) 1_545
B3 N3 4.713(11) .
B4 O10 1.338(8) .
B4 O9 1.355(8) .
B4 O6 1.427(8) .
B4 N3 4.161(11) 1_655
B4 N3 4.308(11) .
B4 N4 4.483(12) 2_566
B4 N4 4.518(11) 1_545
B4 N3 4.575(11) 2_566
B4 N4 4.742(11) 1_445
N1 O13 1.199(13) .
N1 O12 1.265(13) .
N1 O11 1.266(13) .
N1 O13 3.070(16) 2_667
N1 N1 3.075(17) 2_667
N1 O16 3.336(14) 1_655
N1 O12 3.407(12) 2_667
N1 O4 3.420(10) .
N1 O11 3.443(13) 2_667
N2 O16 1.220(10) .
N2 O15 1.255(11) .
N2 O14 1.262(11) .
N2 O22 2.978(13) 1_455
N2 N4 3.178(11) 1_455
N2 O13 3.214(15) 1_455
N2 O20 3.450(12) 1_455
N2 N1 3.527(13) 1_455
N2 O12 3.531(12) 1_455
N3 O19 1.225(10) .
N3 O17 1.245(11) .
N3 O18 1.255(11) .
N3 O19 3.049(12) 2_466
N3 N3 3.328(15) 2_466
N3 O25 3.592(11) 1_455
N3 O26 3.606(10) 2_466
N3 O20 3.627(12) 1_445
N3 O17 3.629(12) 2_466
N4 O22 1.217(11) .
N4 O21 1.256(12) .
N4 O20 1.275(12) .
N4 O16 3.003(13) 1_655
N4 N2 3.178(11) 1_655
N4 O18 3.465(12) 1_665
N4 O15 3.474(11) 1_655
N4 O19 3.596(13) 1_665
N4 O5 3.596(10) .
O1 N2 4.290(9) 1_655
O1 N1 4.724(11) 1_455
O2 Lu1 2.219(4) 2_567
O2 N1 3.911(11) 2_567
O2 N1 4.115(11) 1_455
O3 Lu2 2.209(4) 2_577
O3 N2 3.938(9) 2_577
O3 N1 4.177(11) 1_455
O3 N1 4.732(10) 2_567
O4 N2 4.452(10) 1_655
O5 N2 4.128(9) 1_655
O6 N4 4.269(10) 1_445
O6 N3 4.660(9) 1_655
O6 N4 4.862(10) 1_545
O7 Lu2 2.290(5) 1_545
O7 N2 3.676(10) 1_545
O7 N4 4.177(10) 1_445
O8 Lu4 2.151(5) 1_545
O8 Lu2 2.274(5) 1_545
O8 N2 3.808(9) 1_545
O8 N4 3.910(10) 1_545
O8 N4 4.280(10) 1_445
O9 Lu3 2.203(4) 2_566
O9 N3 3.662(9) 2_566
O9 N3 4.208(9) 1_655
O9 N4 4.724(10) 2_566
O10 Lu4 2.214(5) 1_545
O10 Lu4 2.226(5) 2_566
O10 N4 3.772(10) 1_545
O10 N4 3.926(10) 2_566
O10 N3 4.312(9) 1_655
O10 N4 4.989(10) 1_445
O10 N3 5.005(9) 2_566
O13 N1 3.070(15) 2_667
O13 N2 3.214(15) 1_655
O13 N3 5.064(18) 1_655
O12 N1 3.407(12) 2_667
O12 N2 3.531(12) 1_655
O11 N1 3.443(13) 2_667
O11 N2 4.462(12) 1_655
O11 N3 4.938(12) 1_655
O16 N4 3.003(13) 1_455
O16 N1 3.336(14) 1_455
O15 N4 3.474(11) 1_455
O15 N1 3.636(12) 1_455
O14 N4 3.743(12) 1_455
O14 N1 4.249(13) 1_455
O14 N2 4.973(11) 2_477
O17 N3 3.629(12) 2_466
O17 N4 4.686(13) 1_445
O17 N1 4.916(14) 1_455
O19 N3 3.049(12) 2_466
O19 N4 3.596(13) 1_445
O18 N4 3.465(12) 1_445
O18 N3 3.879(12) 2_466
O18 N4 4.701(13) 2_566
O22 N2 2.978(13) 1_655
O22 N3 3.637(13) 1_665
O22 N4 4.694(15) 2_676
O21 N2 3.764(11) 1_655
O21 N4 4.168(12) 2_676
O21 N3 4.502(12) 1_665
O21 N3 4.715(12) 2_566
O20 N2 3.450(12) 1_655
O20 N3 3.627(12) 1_665
O23 N1 3.746(13) 1_455
O23 N4 3.906(12) 1_445
O23 N1 4.035(13) 2_567
O23 N2 4.196(11) 1_545
O24 N2 3.722(11) 1_655
O24 N2 3.740(10) 2_577
O24 N1 3.933(14) 2_677
O24 N1 4.319(13) 1_565
O25 N3 3.592(11) 1_655
O25 N2 3.652(11) 1_655
O25 N3 3.920(10) 2_566
O26 N3 3.606(10) 2_466
O26 N4 3.609(10) 2_576
O26 N4 3.624(11) 1_455
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
O4 B2 O1 B1 -1.7(12) . . . .
O5 B2 O1 B1 175.4(7) . . . .
Lu3 B2 O1 B1 88(3) . . . .
N3 B2 O1 B1 82.6(8) . . . .
N2 B2 O1 B1 -101.9(7) 1_655 . . .
N1 B2 O1 B1 -51.2(8) . . . .
N4 B2 O1 B1 -144.4(6) . . . .
N2 B2 O1 B1 110.3(8) . . . .
N1 B2 O1 B1 60.4(7) 1_455 . . .
O4 B2 O1 Lu2 -170.4(5) . . . .
O5 B2 O1 Lu2 6.7(12) . . . .
Lu3 B2 O1 Lu2 -80(3) . . . .
N3 B2 O1 Lu2 -86.1(8) . . . .
N2 B2 O1 Lu2 89.4(7) 1_655 . . .
N1 B2 O1 Lu2 140.1(6) . . . .
N4 B2 O1 Lu2 46.9(8) . . . .
N2 B2 O1 Lu2 -58.4(5) . . . .
N1 B2 O1 Lu2 -108.3(7) 1_455 . . .
O4 B2 O1 N2 -112.0(7) . . . .
O5 B2 O1 N2 65.2(9) . . . .
Lu3 B2 O1 N2 -22(3) . . . .
N3 B2 O1 N2 -27.7(6) . . . .
N2 B2 O1 N2 147.9(3) 1_655 . . .
N1 B2 O1 N2 -161.5(3) . . . .
N4 B2 O1 N2 105.3(4) . . . .
N1 B2 O1 N2 -49.8(3) 1_455 . . .
O4 B2 O1 N2 100.1(8) . . . 1_655
O5 B2 O1 N2 -82.7(7) . . . 1_655
Lu3 B2 O1 N2 -170(3) . . . 1_655
N3 B2 O1 N2 -175.6(5) . . . 1_655
N1 B2 O1 N2 50.7(2) . . . 1_655
N4 B2 O1 N2 -42.5(2) . . . 1_655
N2 B2 O1 N2 -147.9(3) . . . 1_655
N1 B2 O1 N2 162.34(19) 1_455 . . 1_655
O4 B2 O1 N1 49.5(7) . . . .
O5 B2 O1 N1 -133.3(8) . . . .
Lu3 B2 O1 N1 140(3) . . . .
N3 B2 O1 N1 133.8(5) . . . .
N2 B2 O1 N1 -50.7(2) 1_655 . . .
N4 B2 O1 N1 -93.2(3) . . . .
N2 B2 O1 N1 161.5(3) . . . .
N1 B2 O1 N1 111.7(3) 1_455 . . .
O4 B2 O1 N1 -62.2(8) . . . 1_455
O5 B2 O1 N1 115.0(7) . . . 1_455
Lu3 B2 O1 N1 28(3) . . . 1_455
N3 B2 O1 N1 22.1(5) . . . 1_455
N2 B2 O1 N1 -162.34(19) 1_655 . . 1_455
N1 B2 O1 N1 -111.7(3) . . . 1_455
N4 B2 O1 N1 155.1(2) . . . 1_455
N2 B2 O1 N1 49.8(3) . . . 1_455
O4 B2 O1 N3 -84.3(8) . . . .
O5 B2 O1 N3 92.9(8) . . . .
Lu3 B2 O1 N3 6(2) . . . .
N2 B2 O1 N3 175.6(5) 1_655 . . .
N1 B2 O1 N3 -133.8(5) . . . .
N4 B2 O1 N3 133.0(5) . . . .
N2 B2 O1 N3 27.7(6) . . . .
N1 B2 O1 N3 -22.1(5) 1_455 . . .
O4 B2 O1 N4 142.7(9) . . . .
O5 B2 O1 N4 -40.2(6) . . . .
Lu3 B2 O1 N4 -127(3) . . . .
N3 B2 O1 N4 -133.0(5) . . . .
N2 B2 O1 N4 42.5(2) 1_655 . . .
N1 B2 O1 N4 93.2(3) . . . .
N2 B2 O1 N4 -105.3(4) . . . .
N1 B2 O1 N4 -155.1(2) 1_455 . . .
O2 B1 O1 B2 3.9(12) . . . .
O3 B1 O1 B2 -176.1(7) . . . .
Lu2 B1 O1 B2 -172.9(8) . . . .
N2 B1 O1 B2 -127.2(7) . . . .
N1 B1 O1 B2 -86.4(7) 1_455 . . .
N1 B1 O1 B2 44.6(7) . . . .
N1 B1 O1 B2 -62.5(11) 2_567 . . .
N2 B1 O1 B2 129.2(6) 2_577 . . .
N2 B1 O1 B2 81.5(7) 1_655 . . .
O2 B1 O1 Lu2 176.7(7) . . . .
O3 B1 O1 Lu2 -3.2(6) . . . .
N2 B1 O1 Lu2 45.64(16) . . . .
N1 B1 O1 Lu2 86.5(3) 1_455 . . .
N1 B1 O1 Lu2 -142.6(2) . . . .
N1 B1 O1 Lu2 110.4(6) 2_567 . . .
N2 B1 O1 Lu2 -57.9(3) 2_577 . . .
N2 B1 O1 Lu2 -105.6(3) 1_655 . . .
O2 B1 O1 N2 131.1(8) . . . .
O3 B1 O1 N2 -48.8(6) . . . .
Lu2 B1 O1 N2 -45.64(17) . . . .
N1 B1 O1 N2 40.9(3) 1_455 . . .
N1 B1 O1 N2 171.8(2) . . . .
N1 B1 O1 N2 64.8(7) 2_567 . . .
N2 B1 O1 N2 -103.5(3) 2_577 . . .
N2 B1 O1 N2 -151.3(3) 1_655 . . .
O2 B1 O1 N2 -77.6(8) . . . 1_655
O3 B1 O1 N2 102.4(6) . . . 1_655
Lu2 B1 O1 N2 105.6(3) . . . 1_655
N2 B1 O1 N2 151.3(3) . . . 1_655
N1 B1 O1 N2 -167.9(2) 1_455 . . 1_655
N1 B1 O1 N2 -36.9(3) . . . 1_655
N1 B1 O1 N2 -144.0(6) 2_567 . . 1_655
N2 B1 O1 N2 47.7(4) 2_577 . . 1_655
O2 B1 O1 N1 -40.7(7) . . . .
O3 B1 O1 N1 139.4(6) . . . .
Lu2 B1 O1 N1 142.6(2) . . . .
N2 B1 O1 N1 -171.8(2) . . . .
N1 B1 O1 N1 -130.9(4) 1_455 . . .
N1 B1 O1 N1 -107.0(6) 2_567 . . .
N2 B1 O1 N1 84.7(3) 2_577 . . .
N2 B1 O1 N1 36.9(3) 1_655 . . .
O2 B1 O1 N1 90.2(8) . . . 1_455
O3 B1 O1 N1 -89.7(6) . . . 1_455
Lu2 B1 O1 N1 -86.5(3) . . . 1_455
N2 B1 O1 N1 -40.9(3) . . . 1_455
N1 B1 O1 N1 130.9(4) . . . 1_455
N1 B1 O1 N1 23.9(6) 2_567 . . 1_455
N2 B1 O1 N1 -144.4(4) 2_577 . . 1_455
N2 B1 O1 N1 167.9(2) 1_655 . . 1_455
O2 B1 O1 N3 50.7(9) . . . .
O3 B1 O1 N3 -129.2(5) . . . .
Lu2 B1 O1 N3 -126.0(3) . . . .
N2 B1 O1 N3 -80.4(3) . . . .
N1 B1 O1 N3 -39.5(4) 1_455 . . .
N1 B1 O1 N3 91.4(3) . . . .
N1 B1 O1 N3 -15.6(8) 2_567 . . .
N2 B1 O1 N3 176.09(18) 2_577 . . .
N2 B1 O1 N3 128.3(4) 1_655 . . .
O2 B1 O1 N4 -97.4(9) . . . .
O3 B1 O1 N4 82.6(9) . . . .
Lu2 B1 O1 N4 85.8(6) . . . .
N2 B1 O1 N4 131.5(7) . . . .
N1 B1 O1 N4 172.3(5) 1_455 . . .
N1 B1 O1 N4 -56.7(7) . . . .
N1 B1 O1 N4 -163.8(4) 2_567 . . .
N2 B1 O1 N4 27.9(8) 2_577 . . .
N2 B1 O1 N4 -19.8(5) 1_655 . . .
O3 B1 O2 Lu1 -5.7(11) . . . 2_567
O1 B1 O2 Lu1 174.4(5) . . . 2_567
N2 B1 O2 Lu1 -85.5(7) . . . 2_567
N1 B1 O2 Lu1 -81.1(5) 1_455 . . 2_567
N1 B1 O2 Lu1 124.3(6) . . . 2_567
N1 B1 O2 Lu1 -51.0(4) 2_567 . . 2_567
N2 B1 O2 Lu1 46.6(6) 2_577 . . 2_567
N2 B1 O2 Lu1 121.3(4) 1_655 . . 2_567
O3 B1 O2 Lu1 -173.0(5) . . . .
O1 B1 O2 Lu1 7.1(11) . . . .
N2 B1 O2 Lu1 107.2(6) . . . .
N1 B1 O2 Lu1 111.6(5) 1_455 . . .
N1 B1 O2 Lu1 -43.0(4) . . . .
N1 B1 O2 Lu1 141.7(7) 2_567 . . .
N2 B1 O2 Lu1 -120.7(4) 2_577 . . .
N2 B1 O2 Lu1 -46.0(6) 1_655 . . .
O3 B1 O2 N1 45.3(9) . . . 2_567
O1 B1 O2 N1 -134.7(6) . . . 2_567
N2 B1 O2 N1 -34.5(6) . . . 2_567
N1 B1 O2 N1 -30.1(4) 1_455 . . 2_567
N1 B1 O2 N1 175.3(4) . . . 2_567
N2 B1 O2 N1 97.5(4) 2_577 . . 2_567
N2 B1 O2 N1 172.3(2) 1_655 . . 2_567
O3 B1 O2 N1 -130.0(7) . . . .
O1 B1 O2 N1 50.0(8) . . . .
N2 B1 O2 N1 150.2(4) . . . .
N1 B1 O2 N1 154.6(4) 1_455 . . .
N1 B1 O2 N1 -175.3(4) 2_567 . . .
N2 B1 O2 N1 -77.8(3) 2_577 . . .
N2 B1 O2 N1 -3.0(3) 1_655 . . .
O3 B1 O2 N1 75.4(8) . . . 1_455
O1 B1 O2 N1 -104.6(7) . . . 1_455
N2 B1 O2 N1 -4.4(5) . . . 1_455
N1 B1 O2 N1 -154.6(4) . . . 1_455
N1 B1 O2 N1 30.1(4) 2_567 . . 1_455
N2 B1 O2 N1 127.6(3) 2_577 . . 1_455
N2 B1 O2 N1 -157.6(3) 1_655 . . 1_455
O3 B1 O2 N2 79.8(8) . . . .
O1 B1 O2 N2 -100.2(9) . . . .
N1 B1 O2 N2 4.4(5) 1_455 . . .
N1 B1 O2 N2 -150.2(4) . . . .
N1 B1 O2 N2 34.5(6) 2_567 . . .
N2 B1 O2 N2 132.0(6) 2_577 . . .
N2 B1 O2 N2 -153.2(6) 1_655 . . .
O2 B1 O3 Lu2 38.1(14) . . . 2_577
O1 B1 O3 Lu2 -142.0(6) . . . 2_577
Lu2 B1 O3 Lu2 -145.5(9) . . . 2_577
N2 B1 O3 Lu2 160.8(9) . . . 2_577
N1 B1 O3 Lu2 112.2(8) 1_455 . . 2_577
N1 B1 O3 Lu2 -41.0(12) . . . 2_577
N1 B1 O3 Lu2 71.4(8) 2_567 . . 2_577
N2 B1 O3 Lu2 -42.2(6) 2_577 . . 2_577
N2 B1 O3 Lu2 -83.9(8) 1_655 . . 2_577
O2 B1 O3 Lu2 -176.4(7) . . . .
O1 B1 O3 Lu2 3.5(7) . . . .
N2 B1 O3 Lu2 -53.66(19) . . . .
N1 B1 O3 Lu2 -102.3(2) 1_455 . . .
N1 B1 O3 Lu2 104.5(6) . . . .
N1 B1 O3 Lu2 -143.1(2) 2_567 . . .
N2 B1 O3 Lu2 103.3(3) 2_577 . . .
N2 B1 O3 Lu2 61.6(4) 1_655 . . .
O2 B1 O3 N2 -122.8(7) . . . .
O1 B1 O3 N2 57.2(6) . . . .
Lu2 B1 O3 N2 53.66(19) . . . .
N1 B1 O3 N2 -48.7(2) 1_455 . . .
N1 B1 O3 N2 158.2(5) . . . .
N1 B1 O3 N2 -89.5(2) 2_567 . . .
N2 B1 O3 N2 157.0(3) 2_577 . . .
N2 B1 O3 N2 115.3(3) 1_655 . . .
O2 B1 O3 N2 80.2(8) . . . 2_577
O1 B1 O3 N2 -99.8(6) . . . 2_577
Lu2 B1 O3 N2 -103.3(3) . . . 2_577
N2 B1 O3 N2 -157.0(3) . . . 2_577
N1 B1 O3 N2 154.3(3) 1_455 . . 2_577
N1 B1 O3 N2 1.2(8) . . . 2_577
N1 B1 O3 N2 113.5(3) 2_567 . . 2_577
N2 B1 O3 N2 -41.7(4) 1_655 . . 2_577
O2 B1 O3 N1 -74.1(8) . . . 1_455
O1 B1 O3 N1 105.8(6) . . . 1_455
Lu2 B1 O3 N1 102.3(2) . . . 1_455
N2 B1 O3 N1 48.7(2) . . . 1_455
N1 B1 O3 N1 -153.1(7) . . . 1_455
N1 B1 O3 N1 -40.8(2) 2_567 . . 1_455
N2 B1 O3 N1 -154.3(3) 2_577 . . 1_455
N2 B1 O3 N1 164.0(3) 1_655 . . 1_455
O2 B1 O3 N1 -33.3(7) . . . 2_567
O1 B1 O3 N1 146.6(6) . . . 2_567
Lu2 B1 O3 N1 143.1(2) . . . 2_567
N2 B1 O3 N1 89.5(2) . . . 2_567
N1 B1 O3 N1 40.8(2) 1_455 . . 2_567
N1 B1 O3 N1 -112.3(6) . . . 2_567
N2 B1 O3 N1 -113.5(3) 2_577 . . 2_567
N2 B1 O3 N1 -155.3(3) 1_655 . . 2_567
O5 B2 O4 Lu1 170.6(5) . . . .
O1 B2 O4 Lu1 -12.1(12) . . . .
Lu3 B2 O4 Lu1 -179.3(7) . . . .
N3 B2 O4 Lu1 -128.5(6) . . . .
N2 B2 O4 Lu1 83.7(6) 1_655 . . .
N1 B2 O4 Lu1 61.7(5) . . . .
N4 B2 O4 Lu1 121.9(5) . . . .
N2 B2 O4 Lu1 -66.2(8) . . . .
N1 B2 O4 Lu1 -60.6(6) 1_455 . . .
O5 B2 O4 Lu3 -10.1(7) . . . .
O1 B2 O4 Lu3 167.2(7) . . . .
N3 B2 O4 Lu3 50.75(17) . . . .
N2 B2 O4 Lu3 -97.0(2) 1_655 . . .
N1 B2 O4 Lu3 -119.1(4) . . . .
N4 B2 O4 Lu3 -58.8(5) . . . .
N2 B2 O4 Lu3 113.1(4) . . . .
N1 B2 O4 Lu3 118.6(2) 1_455 . . .
O5 B2 O4 N1 108.9(6) . . . .
O1 B2 O4 N1 -73.8(8) . . . .
Lu3 B2 O4 N1 119.1(4) . . . .
N3 B2 O4 N1 169.8(3) . . . .
N2 B2 O4 N1 22.0(4) 1_655 . . .
N4 B2 O4 N1 60.3(5) . . . .
N2 B2 O4 N1 -127.8(4) . . . .
N1 B2 O4 N1 -122.3(3) 1_455 . . .
O5 B2 O4 N3 -60.9(7) . . . .
O1 B2 O4 N3 116.4(7) . . . .
Lu3 B2 O4 N3 -50.75(17) . . . .
N2 B2 O4 N3 -147.8(2) 1_655 . . .
N1 B2 O4 N3 -169.8(3) . . . .
N4 B2 O4 N3 -109.6(4) . . . .
N2 B2 O4 N3 62.3(4) . . . .
N1 B2 O4 N3 67.9(2) 1_455 . . .
O5 B2 O4 N2 86.9(7) . . . 1_655
O1 B2 O4 N2 -95.8(8) . . . 1_655
Lu3 B2 O4 N2 97.0(2) . . . 1_655
N3 B2 O4 N2 147.8(2) . . . 1_655
N1 B2 O4 N2 -22.0(4) . . . 1_655
N4 B2 O4 N2 38.2(3) . . . 1_655
N2 B2 O4 N2 -149.9(6) . . . 1_655
N1 B2 O4 N2 -144.3(3) 1_455 . . 1_655
O4 B2 O5 Lu4 179.0(5) . . . .
O1 B2 O5 Lu4 1.6(13) . . . .
Lu3 B2 O5 Lu4 169.2(8) . . . .
N3 B2 O5 Lu4 122.4(7) . . . .
N2 B2 O5 Lu4 -84.8(7) 1_655 . . .
N1 B2 O5 Lu4 -122.5(6) . . . .
N4 B2 O5 Lu4 -68.1(6) . . . .
N2 B2 O5 Lu4 40.5(8) . . . .
N1 B2 O5 Lu4 71.8(9) 1_455 . . .
O4 B2 O5 Lu3 9.8(7) . . . .
O1 B2 O5 Lu3 -167.5(7) . . . .
N3 B2 O5 Lu3 -46.76(16) . . . .
N2 B2 O5 Lu3 106.1(2) 1_655 . . .
N1 B2 O5 Lu3 68.3(4) . . . .
N4 B2 O5 Lu3 122.7(4) . . . .
N2 B2 O5 Lu3 -128.7(2) . . . .
N1 B2 O5 Lu3 -97.4(4) 1_455 . . .
O4 B2 O5 N4 -112.9(7) . . . .
O1 B2 O5 N4 69.8(8) . . . .
Lu3 B2 O5 N4 -122.7(4) . . . .
N3 B2 O5 N4 -169.5(4) . . . .
N2 B2 O5 N4 -16.6(4) 1_655 . . .
N1 B2 O5 N4 -54.4(6) . . . .
N2 B2 O5 N4 108.6(4) . . . .
N1 B2 O5 N4 139.9(4) 1_455 . . .
O4 B2 O5 N3 56.6(7) . . . .
O1 B2 O5 N3 -120.8(7) . . . .
Lu3 B2 O5 N3 46.76(16) . . . .
N2 B2 O5 N3 152.8(2) 1_655 . . .
N1 B2 O5 N3 115.1(4) . . . .
N4 B2 O5 N3 169.5(4) . . . .
N2 B2 O5 N3 -81.9(2) . . . .
N1 B2 O5 N3 -50.6(4) 1_455 . . .
O4 B2 O5 N2 -96.2(7) . . . 1_655
O1 B2 O5 N2 86.4(7) . . . 1_655
Lu3 B2 O5 N2 -106.1(2) . . . 1_655
N3 B2 O5 N2 -152.8(2) . . . 1_655
N1 B2 O5 N2 -37.7(4) . . . 1_655
N4 B2 O5 N2 16.6(4) . . . 1_655
N2 B2 O5 N2 125.3(3) . . . 1_655
N1 B2 O5 N2 156.5(4) 1_455 . . 1_655
O4 B2 O5 N1 -58.5(6) . . . .
O1 B2 O5 N1 124.1(9) . . . .
Lu3 B2 O5 N1 -68.3(4) . . . .
N3 B2 O5 N1 -115.1(4) . . . .
N2 B2 O5 N1 37.7(4) 1_655 . . .
N4 B2 O5 N1 54.4(6) . . . .
N2 B2 O5 N1 163.0(5) . . . .
N1 B2 O5 N1 -165.7(7) 1_455 . . .
O4 B2 O5 N2 138.5(8) . . . .
O1 B2 O5 N2 -38.9(6) . . . .
Lu3 B2 O5 N2 128.7(2) . . . .
N3 B2 O5 N2 81.9(2) . . . .
N2 B2 O5 N2 -125.3(3) 1_655 . . .
N1 B2 O5 N2 -163.0(5) . . . .
N4 B2 O5 N2 -108.6(4) . . . .
N1 B2 O5 N2 31.2(3) 1_455 . . .
O7 B3 O6 B4 -174.9(7) . . . .
O8 B3 O6 B4 3.1(12) . . . .
N4 B3 O6 B4 -88.6(7) 1_445 . . .
N2 B3 O6 B4 -92.1(8) 1_545 . . .
N1 B3 O6 B4 133.1(7) . . . .
N4 B3 O6 B4 42.5(7) 1_545 . . .
N3 B3 O6 B4 -119.4(8) . . . .
O7 B3 O6 Lu3 -4.9(13) . . . .
O8 B3 O6 Lu3 173.0(5) . . . .
N4 B3 O6 Lu3 81.4(7) 1_445 . . .
N2 B3 O6 Lu3 77.9(9) 1_545 . . .
N1 B3 O6 Lu3 -57.0(7) . . . .
N4 B3 O6 Lu3 -147.5(6) 1_545 . . .
N3 B3 O6 Lu3 50.6(6) . . . .
O7 B3 O6 N3 -55.5(8) . . . .
O8 B3 O6 N3 122.4(7) . . . .
N4 B3 O6 N3 30.8(3) 1_445 . . .
N2 B3 O6 N3 27.3(7) 1_545 . . .
N1 B3 O6 N3 -107.5(3) . . . .
N4 B3 O6 N3 161.9(2) 1_545 . . .
O7 B3 O6 N4 -86.3(7) . . . 1_445
O8 B3 O6 N4 91.6(8) . . . 1_445
N2 B3 O6 N4 -3.5(5) 1_545 . . 1_445
N1 B3 O6 N4 -138.3(3) . . . 1_445
N4 B3 O6 N4 131.1(3) 1_545 . . 1_445
N3 B3 O6 N4 -30.8(3) . . . 1_445
O7 B3 O6 N1 52.0(7) . . . .
O8 B3 O6 N1 -130.0(8) . . . .
N4 B3 O6 N1 138.3(3) 1_445 . . .
N2 B3 O6 N1 134.8(6) 1_545 . . .
N4 B3 O6 N1 -90.6(2) 1_545 . . .
N3 B3 O6 N1 107.5(3) . . . .
O7 B3 O6 N3 116.3(7) . . . 1_655
O8 B3 O6 N3 -65.7(8) . . . 1_655
N4 B3 O6 N3 -157.4(2) 1_445 . . 1_655
N2 B3 O6 N3 -160.9(4) 1_545 . . 1_655
N1 B3 O6 N3 64.3(3) . . . 1_655
N4 B3 O6 N3 -26.3(3) 1_545 . . 1_655
N3 B3 O6 N3 171.8(5) . . . 1_655
O7 B3 O6 N4 142.6(8) . . . 1_545
O8 B3 O6 N4 -39.4(7) . . . 1_545
N4 B3 O6 N4 -131.1(3) 1_445 . . 1_545
N2 B3 O6 N4 -134.6(6) 1_545 . . 1_545
N1 B3 O6 N4 90.6(2) . . . 1_545
N3 B3 O6 N4 -161.9(2) . . . 1_545
O10 B4 O6 B3 -0.8(11) . . . .
O9 B4 O6 B3 178.3(7) . . . .
Lu3 B4 O6 B3 174.0(8) . . . .
N3 B4 O6 B3 -95.0(7) 1_655 . . .
N3 B4 O6 B3 127.7(7) . . . .
N4 B4 O6 B3 69.5(8) 2_566 . . .
N4 B4 O6 B3 -44.2(7) 1_545 . . .
N3 B4 O6 B3 -136.7(6) 2_566 . . .
N4 B4 O6 B3 73.6(7) 1_445 . . .
O10 B4 O6 Lu3 -174.8(7) . . . .
O9 B4 O6 Lu3 4.3(6) . . . .
N3 B4 O6 Lu3 91.0(2) 1_655 . . .
N3 B4 O6 Lu3 -46.32(14) . . . .
N4 B4 O6 Lu3 -104.5(4) 2_566 . . .
N4 B4 O6 Lu3 141.8(2) 1_545 . . .
N3 B4 O6 Lu3 49.3(4) 2_566 . . .
N4 B4 O6 Lu3 -100.4(2) 1_445 . . .
O10 B4 O6 N3 -128.5(7) . . . .
O9 B4 O6 N3 50.6(6) . . . .
Lu3 B4 O6 N3 46.32(14) . . . .
N3 B4 O6 N3 137.3(3) 1_655 . . .
N4 B4 O6 N3 -58.2(4) 2_566 . . .
N4 B4 O6 N3 -171.87(19) 1_545 . . .
N3 B4 O6 N3 95.6(4) 2_566 . . .
N4 B4 O6 N3 -54.10(19) 1_445 . . .
O10 B4 O6 N4 -74.4(7) . . . 1_445
O9 B4 O6 N4 104.7(6) . . . 1_445
Lu3 B4 O6 N4 100.4(2) . . . 1_445
N3 B4 O6 N4 -168.57(19) 1_655 . . 1_445
N3 B4 O6 N4 54.10(19) . . . 1_445
N4 B4 O6 N4 -4.1(5) 2_566 . . 1_445
N4 B4 O6 N4 -117.8(2) 1_545 . . 1_445
N3 B4 O6 N4 149.7(3) 2_566 . . 1_445
O10 B4 O6 N1 105.5(7) . . . .
O9 B4 O6 N1 -75.4(7) . . . .
Lu3 B4 O6 N1 -79.7(4) . . . .
N3 B4 O6 N1 11.3(5) 1_655 . . .
N3 B4 O6 N1 -126.1(5) . . . .
N4 B4 O6 N1 175.7(2) 2_566 . . .
N4 B4 O6 N1 62.1(5) 1_545 . . .
N3 B4 O6 N1 -30.5(7) 2_566 . . .
N4 B4 O6 N1 179.8(5) 1_445 . . .
O10 B4 O6 N3 94.2(7) . . . 1_655
O9 B4 O6 N3 -86.7(6) . . . 1_655
Lu3 B4 O6 N3 -91.0(2) . . . 1_655
N3 B4 O6 N3 -137.3(3) . . . 1_655
N4 B4 O6 N3 164.4(5) 2_566 . . 1_655
N4 B4 O6 N3 50.8(2) 1_545 . . 1_655
N3 B4 O6 N3 -41.7(3) 2_566 . . 1_655
N4 B4 O6 N3 168.57(19) 1_445 . . 1_655
O10 B4 O6 N4 43.4(6) . . . 1_545
O9 B4 O6 N4 -137.5(7) . . . 1_545
Lu3 B4 O6 N4 -141.8(2) . . . 1_545
N3 B4 O6 N4 -50.8(2) 1_655 . . 1_545
N3 B4 O6 N4 171.87(19) . . . 1_545
N4 B4 O6 N4 113.6(4) 2_566 . . 1_545
N3 B4 O6 N4 -92.5(4) 2_566 . . 1_545
N4 B4 O6 N4 117.8(2) 1_445 . . 1_545
O8 B3 O7 Lu1 156.4(5) . . . .
O6 B3 O7 Lu1 -25.5(11) . . . .
Lu2 B3 O7 Lu1 154.3(7) 1_545 . . .
N4 B3 O7 Lu1 -113.7(6) 1_445 . . .
N2 B3 O7 Lu1 -155.4(7) 1_545 . . .
N1 B3 O7 Lu1 38.9(5) . . . .
N4 B3 O7 Lu1 98.7(7) 1_545 . . .
N3 B3 O7 Lu1 -64.0(6) . . . .
O8 B3 O7 Lu2 2.0(7) . . . 1_545
O6 B3 O7 Lu2 -179.8(7) . . . 1_545
N4 B3 O7 Lu2 92.0(2) 1_445 . . 1_545
N2 B3 O7 Lu2 50.21(17) 1_545 . . 1_545
N1 B3 O7 Lu2 -115.4(3) . . . 1_545
N4 B3 O7 Lu2 -55.7(6) 1_545 . . 1_545
N3 B3 O7 Lu2 141.7(2) . . . 1_545
O8 B3 O7 N2 -48.2(7) . . . 1_545
O6 B3 O7 N2 129.9(7) . . . 1_545
Lu2 B3 O7 N2 -50.21(17) 1_545 . . 1_545
N4 B3 O7 N2 41.8(2) 1_445 . . 1_545
N1 B3 O7 N2 -165.6(3) . . . 1_545
N4 B3 O7 N2 -105.9(5) 1_545 . . 1_545
N3 B3 O7 N2 91.5(2) . . . 1_545
O8 B3 O7 N1 117.4(6) . . . .
O6 B3 O7 N1 -64.4(7) . . . .
Lu2 B3 O7 N1 115.4(3) 1_545 . . .
N4 B3 O7 N1 -152.6(2) 1_445 . . .
N2 B3 O7 N1 165.6(3) 1_545 . . .
N4 B3 O7 N1 59.8(6) 1_545 . . .
N3 B3 O7 N1 -102.9(2) . . . .
O8 B3 O7 N4 -90.0(7) . . . 1_445
O6 B3 O7 N4 88.2(7) . . . 1_445
Lu2 B3 O7 N4 -92.0(2) 1_545 . . 1_445
N2 B3 O7 N4 -41.8(2) 1_545 . . 1_445
N1 B3 O7 N4 152.6(2) . . . 1_445
N4 B3 O7 N4 -147.7(6) 1_545 . . 1_445
N3 B3 O7 N4 49.66(17) . . . 1_445
O8 B3 O7 N3 -139.6(7) . . . .
O6 B3 O7 N3 38.5(6) . . . .
Lu2 B3 O7 N3 -141.7(2) 1_545 . . .
N4 B3 O7 N3 -49.66(17) 1_445 . . .
N2 B3 O7 N3 -91.5(2) 1_545 . . .
N1 B3 O7 N3 102.9(2) . . . .
N4 B3 O7 N3 162.7(6) 1_545 . . .
O7 B3 O8 Lu4 -176.6(5) . . . 1_545
O6 B3 O8 Lu4 5.3(12) . . . 1_545
Lu2 B3 O8 Lu4 -174.6(7) 1_545 . . 1_545
N4 B3 O8 Lu4 96.3(6) 1_445 . . 1_545
N2 B3 O8 Lu4 137.8(6) 1_545 . . 1_545
N1 B3 O8 Lu4 -106.1(5) . . . 1_545
N4 B3 O8 Lu4 -50.8(4) 1_545 . . 1_545
N3 B3 O8 Lu4 68.9(9) . . . 1_545
O7 B3 O8 Lu2 -2.0(7) . . . 1_545
O6 B3 O8 Lu2 179.9(7) . . . 1_545
N4 B3 O8 Lu2 -89.2(2) 1_445 . . 1_545
N2 B3 O8 Lu2 -47.63(16) 1_545 . . 1_545
N1 B3 O8 Lu2 68.5(5) . . . 1_545
N4 B3 O8 Lu2 123.8(4) 1_545 . . 1_545
N3 B3 O8 Lu2 -116.5(5) . . . 1_545
O7 B3 O8 N2 45.6(7) . . . 1_545
O6 B3 O8 N2 -132.5(7) . . . 1_545
Lu2 B3 O8 N2 47.63(16) 1_545 . . 1_545
N4 B3 O8 N2 -41.5(2) 1_445 . . 1_545
N1 B3 O8 N2 116.1(4) . . . 1_545
N4 B3 O8 N2 171.5(3) 1_545 . . 1_545
N3 B3 O8 N2 -68.8(5) . . . 1_545
O7 B3 O8 N4 -125.9(6) . . . 1_545
O6 B3 O8 N4 56.1(9) . . . 1_545
Lu2 B3 O8 N4 -123.8(4) 1_545 . . 1_545
N4 B3 O8 N4 147.0(3) 1_445 . . 1_545
N2 B3 O8 N4 -171.5(3) 1_545 . . 1_545
N1 B3 O8 N4 -55.3(5) . . . 1_545
N3 B3 O8 N4 119.7(5) . . . 1_545
O7 B3 O8 N4 87.1(7) . . . 1_445
O6 B3 O8 N4 -91.0(7) . . . 1_445
Lu2 B3 O8 N4 89.2(2) 1_545 . . 1_445
N2 B3 O8 N4 41.5(2) 1_545 . . 1_445
N1 B3 O8 N4 157.6(5) . . . 1_445
N4 B3 O8 N4 -147.0(3) 1_545 . . 1_445
N3 B3 O8 N4 -27.3(5) . . . 1_445
O10 B4 O9 Lu3 9.4(16) . . . 2_566
O6 B4 O9 Lu3 -169.7(7) . . . 2_566
Lu3 B4 O9 Lu3 -164.9(11) . . . 2_566
N3 B4 O9 Lu3 90.9(10) 1_655 . . 2_566
N3 B4 O9 Lu3 -120.4(10) . . . 2_566
N4 B4 O9 Lu3 -41.0(10) 2_566 . . 2_566
N4 B4 O9 Lu3 71.9(12) 1_545 . . 2_566
N3 B4 O9 Lu3 72.3(9) 2_566 . . 2_566
N4 B4 O9 Lu3 -101.6(9) 1_445 . . 2_566
O10 B4 O9 Lu3 174.3(6) . . . .
O6 B4 O9 Lu3 -4.8(7) . . . .
N3 B4 O9 Lu3 -104.2(2) 1_655 . . .
N3 B4 O9 Lu3 44.47(18) . . . .
N4 B4 O9 Lu3 123.9(2) 2_566 . . .
N4 B4 O9 Lu3 -123.3(4) 1_545 . . .
N3 B4 O9 Lu3 -122.8(5) 2_566 . . .
N4 B4 O9 Lu3 63.2(4) 1_445 . . .
O10 B4 O9 N3 -62.9(9) . . . 2_566
O6 B4 O9 N3 118.0(5) . . . 2_566
Lu3 B4 O9 N3 122.8(5) . . . 2_566
N3 B4 O9 N3 18.6(4) 1_655 . . 2_566
N3 B4 O9 N3 167.3(4) . . . 2_566
N4 B4 O9 N3 -113.3(4) 2_566 . . 2_566
N4 B4 O9 N3 -0.5(7) 1_545 . . 2_566
N4 B4 O9 N3 -173.9(3) 1_445 . . 2_566
O10 B4 O9 N3 129.8(7) . . . .
O6 B4 O9 N3 -49.3(6) . . . .
Lu3 B4 O9 N3 -44.47(18) . . . .
N3 B4 O9 N3 -148.7(2) 1_655 . . .
N4 B4 O9 N3 79.4(2) 2_566 . . .
N4 B4 O9 N3 -167.7(4) 1_545 . . .
N3 B4 O9 N3 -167.3(4) 2_566 . . .
N4 B4 O9 N3 18.8(3) 1_445 . . .
O10 B4 O9 N3 -81.5(7) . . . 1_655
O6 B4 O9 N3 99.4(6) . . . 1_655
Lu3 B4 O9 N3 104.2(2) . . . 1_655
N3 B4 O9 N3 148.7(2) . . . 1_655
N4 B4 O9 N3 -131.9(2) 2_566 . . 1_655
N4 B4 O9 N3 -19.0(4) 1_545 . . 1_655
N3 B4 O9 N3 -18.6(4) 2_566 . . 1_655
N4 B4 O9 N3 167.5(3) 1_445 . . 1_655
O10 B4 O9 N4 50.4(7) . . . 2_566
O6 B4 O9 N4 -128.7(6) . . . 2_566
Lu3 B4 O9 N4 -123.9(2) . . . 2_566
N3 B4 O9 N4 131.9(2) 1_655 . . 2_566
N3 B4 O9 N4 -79.4(2) . . . 2_566
N4 B4 O9 N4 112.9(5) 1_545 . . 2_566
N3 B4 O9 N4 113.3(4) 2_566 . . 2_566
N4 B4 O9 N4 -60.6(3) 1_445 . . 2_566
O9 B4 O10 Lu4 171.5(5) . . . 1_545
O6 B4 O10 Lu4 -9.5(11) . . . 1_545
N3 B4 O10 Lu4 92.4(5) 1_655 . . 1_545
N3 B4 O10 Lu4 -95.7(6) . . . 1_545
N4 B4 O10 Lu4 -122.4(6) 2_566 . . 1_545
N4 B4 O10 Lu4 56.0(4) 1_545 . . 1_545
N3 B4 O10 Lu4 134.9(4) 2_566 . . 1_545
N4 B4 O10 Lu4 -68.1(5) 1_445 . . 1_545
O9 B4 O10 Lu4 -20.2(10) . . . 2_566
O6 B4 O10 Lu4 158.8(5) . . . 2_566
N3 B4 O10 Lu4 -99.3(4) 1_655 . . 2_566
N3 B4 O10 Lu4 72.6(7) . . . 2_566
N4 B4 O10 Lu4 45.9(3) 2_566 . . 2_566
N4 B4 O10 Lu4 -135.7(6) 1_545 . . 2_566
N3 B4 O10 Lu4 -56.8(5) 2_566 . . 2_566
N4 B4 O10 Lu4 100.2(4) 1_445 . . 2_566
O9 B4 O10 N4 115.4(7) . . . 1_545
O6 B4 O10 N4 -65.6(8) . . . 1_545
N3 B4 O10 N4 36.4(3) 1_655 . . 1_545
N3 B4 O10 N4 -151.7(4) . . . 1_545
N4 B4 O10 N4 -178.4(4) 2_566 . . 1_545
N3 B4 O10 N4 78.9(3) 2_566 . . 1_545
N4 B4 O10 N4 -124.2(3) 1_445 . . 1_545
O9 B4 O10 N4 -66.1(8) . . . 2_566
O6 B4 O10 N4 112.9(6) . . . 2_566
N3 B4 O10 N4 -145.2(2) 1_655 . . 2_566
N3 B4 O10 N4 26.7(6) . . . 2_566
N4 B4 O10 N4 178.4(4) 1_545 . . 2_566
N3 B4 O10 N4 -102.7(3) 2_566 . . 2_566
N4 B4 O10 N4 54.3(3) 1_445 . . 2_566
O9 B4 O10 N3 79.1(7) . . . 1_655
O6 B4 O10 N3 -101.9(7) . . . 1_655
N3 B4 O10 N3 171.9(6) . . . 1_655
N4 B4 O10 N3 145.2(2) 2_566 . . 1_655
N4 B4 O10 N3 -36.4(3) 1_545 . . 1_655
N3 B4 O10 N3 42.6(2) 2_566 . . 1_655
N4 B4 O10 N3 -160.5(2) 1_445 . . 1_655
O9 B4 O10 N4 -120.4(8) . . . 1_445
O6 B4 O10 N4 58.6(6) . . . 1_445
N3 B4 O10 N4 160.5(2) 1_655 . . 1_445
N3 B4 O10 N4 -27.6(4) . . . 1_445
N4 B4 O10 N4 -54.3(3) 2_566 . . 1_445
N4 B4 O10 N4 124.2(3) 1_545 . . 1_445
N3 B4 O10 N4 -156.9(3) 2_566 . . 1_445
O9 B4 O10 N3 36.5(6) . . . 2_566
O6 B4 O10 N3 -144.5(8) . . . 2_566
N3 B4 O10 N3 -42.6(2) 1_655 . . 2_566
N3 B4 O10 N3 129.3(6) . . . 2_566
N4 B4 O10 N3 102.7(3) 2_566 . . 2_566
N4 B4 O10 N3 -78.9(3) 1_545 . . 2_566
N4 B4 O10 N3 156.9(3) 1_445 . . 2_566
O12 N1 O13 N1 87.5(10) . . . 2_667
O11 N1 O13 N1 -89.7(10) . . . 2_667
O13 N1 O13 N1 0.0010(10) 2_667 . . 2_667
O16 N1 O13 N1 149.6(6) 1_655 . . 2_667
O12 N1 O13 N1 -19.8(4) 2_667 . . 2_667
O4 N1 O13 N1 178.1(15) . . . 2_667
O11 N1 O13 N1 19.6(4) 2_667 . . 2_667
O12 N1 O13 N2 -58.4(11) . . . 1_655
O11 N1 O13 N2 124.4(9) . . . 1_655
O13 N1 O13 N2 -145.9(6) 2_667 . . 1_655
N1 N1 O13 N2 -145.9(6) 2_667 . . 1_655
O16 N1 O13 N2 3.7(4) 1_655 . . 1_655
O12 N1 O13 N2 -165.7(7) 2_667 . . 1_655
O4 N1 O13 N2 32.2(16) . . . 1_655
O11 N1 O13 N2 -126.3(6) 2_667 . . 1_655
O12 N1 O13 N3 -147.5(9) . . . 1_655
O11 N1 O13 N3 35.3(11) . . . 1_655
O13 N1 O13 N3 125.0(5) 2_667 . . 1_655
N1 N1 O13 N3 125.0(5) 2_667 . . 1_655
O16 N1 O13 N3 -85.4(4) 1_655 . . 1_655
O12 N1 O13 N3 105.3(5) 2_667 . . 1_655
O4 N1 O13 N3 -56.9(15) . . . 1_655
O11 N1 O13 N3 144.6(5) 2_667 . . 1_655
O13 N1 O12 Lu1 177.8(10) . . . .
O11 N1 O12 Lu1 -4.8(9) . . . .
O13 N1 O12 Lu1 -84.1(4) 2_667 . . .
N1 N1 O12 Lu1 -103.2(5) 2_667 . . .
O16 N1 O12 Lu1 107.9(3) 1_655 . . .
O12 N1 O12 Lu1 -103.2(5) 2_667 . . .
O4 N1 O12 Lu1 42.93(18) . . . .
O11 N1 O12 Lu1 -122.5(3) 2_667 . . .
O13 N1 O12 N1 -79.0(11) . . . 2_667
O11 N1 O12 N1 98.4(9) . . . 2_667
Lu1 N1 O12 N1 103.2(5) . . . 2_667
O13 N1 O12 N1 19.0(4) 2_667 . . 2_667
O16 N1 O12 N1 -148.9(5) 1_655 . . 2_667
O12 N1 O12 N1 0 2_667 . . 2_667
O4 N1 O12 N1 146.1(4) . . . 2_667
O11 N1 O12 N1 -19.3(3) 2_667 . . 2_667
O13 N1 O12 N2 51.8(11) . . . 1_655
O11 N1 O12 N2 -130.9(9) . . . 1_655
Lu1 N1 O12 N2 -126.1(3) . . . 1_655
O13 N1 O12 N2 149.8(4) 2_667 . . 1_655
N1 N1 O12 N2 130.8(5) 2_667 . . 1_655
O16 N1 O12 N2 -18.1(2) 1_655 . . 1_655
O12 N1 O12 N2 130.8(5) 2_667 . . 1_655
O4 N1 O12 N2 -83.1(3) . . . 1_655
O11 N1 O12 N2 111.4(3) 2_667 . . 1_655
O13 N1 O11 Lu1 -177.7(10) . . . .
O12 N1 O11 Lu1 4.9(9) . . . .
O13 N1 O11 Lu1 83.1(4) 2_667 . . .
N1 N1 O11 Lu1 102.2(5) 2_667 . . .
O16 N1 O11 Lu1 -74.6(6) 1_655 . . .
O12 N1 O11 Lu1 121.7(4) 2_667 . . .
O4 N1 O11 Lu1 -42.3(2) . . . .
O11 N1 O11 Lu1 102.2(5) 2_667 . . .
O13 N1 O11 N1 80.1(11) . . . 2_667
O12 N1 O11 N1 -97.3(10) . . . 2_667
Lu1 N1 O11 N1 -102.2(5) . . . 2_667
O13 N1 O11 N1 -19.1(4) 2_667 . . 2_667
O16 N1 O11 N1 -176.8(9) 1_655 . . 2_667
O12 N1 O11 N1 19.5(3) 2_667 . . 2_667
O4 N1 O11 N1 -144.5(4) . . . 2_667
O11 N1 O11 N1 -0.0010(10) 2_667 . . 2_667
O13 N1 O11 N2 -83.8(13) . . . 1_655
O12 N1 O11 N2 98.8(11) . . . 1_655
Lu1 N1 O11 N2 93.9(8) . . . 1_655
O13 N1 O11 N2 177.0(9) 2_667 . . 1_655
N1 N1 O11 N2 -163.9(11) 2_667 . . 1_655
O16 N1 O11 N2 19.3(4) 1_655 . . 1_655
O12 N1 O11 N2 -144.4(8) 2_667 . . 1_655
O4 N1 O11 N2 51.6(8) . . . 1_655
O11 N1 O11 N2 -163.9(11) 2_667 . . 1_655
O13 N1 O11 N3 -37.1(12) . . . 1_655
O12 N1 O11 N3 145.5(7) . . . 1_655
Lu1 N1 O11 N3 140.6(5) . . . 1_655
O13 N1 O11 N3 -136.3(3) 2_667 . . 1_655
N1 N1 O11 N3 -117.2(4) 2_667 . . 1_655
O16 N1 O11 N3 66.1(6) 1_655 . . 1_655
O12 N1 O11 N3 -97.7(3) 2_667 . . 1_655
O4 N1 O11 N3 98.4(3) . . . 1_655
O11 N1 O11 N3 -117.2(4) 2_667 . . 1_655
O15 N2 O16 N4 -80.9(9) . . . 1_455
O14 N2 O16 N4 97.8(9) . . . 1_455
O22 N2 O16 N4 -1.9(4) 1_455 . . 1_455
O13 N2 O16 N4 -148.3(4) 1_455 . . 1_455
O20 N2 O16 N4 21.7(3) 1_455 . . 1_455
N1 N2 O16 N4 -151.9(5) 1_455 . . 1_455
O12 N2 O16 N4 -171.7(6) 1_455 . . 1_455
O15 N2 O16 N1 71.0(9) . . . 1_455
O14 N2 O16 N1 -110.3(9) . . . 1_455
O22 N2 O16 N1 150.0(4) 1_455 . . 1_455
N4 N2 O16 N1 151.9(5) 1_455 . . 1_455
O13 N2 O16 N1 3.6(4) 1_455 . . 1_455
O20 N2 O16 N1 173.6(5) 1_455 . . 1_455
O12 N2 O16 N1 -19.9(3) 1_455 . . 1_455
O16 N2 O15 Lu2 178.0(8) . . . .
O14 N2 O15 Lu2 -0.8(8) . . . .
O22 N2 O15 Lu2 91.3(3) 1_455 . . .
N4 N2 O15 Lu2 109.2(3) 1_455 . . .
O13 N2 O15 Lu2 -104.0(4) 1_455 . . .
O20 N2 O15 Lu2 107.2(4) 1_455 . . .
N1 N2 O15 Lu2 -118.1(3) 1_455 . . .
O12 N2 O15 Lu2 -116.7(3) 1_455 . . .
O16 N2 O15 N4 68.9(8) . . . 1_455
O14 N2 O15 N4 -110.0(8) . . . 1_455
Lu2 N2 O15 N4 -109.2(3) . . . 1_455
O22 N2 O15 N4 -17.9(3) 1_455 . . 1_455
O13 N2 O15 N4 146.9(4) 1_455 . . 1_455
O20 N2 O15 N4 -2.0(3) 1_455 . . 1_455
N1 N2 O15 N4 132.7(4) 1_455 . . 1_455
O12 N2 O15 N4 134.1(4) 1_455 . . 1_455
O16 N2 O15 N1 -63.8(9) . . . 1_455
O14 N2 O15 N1 117.3(8) . . . 1_455
Lu2 N2 O15 N1 118.1(3) . . . 1_455
O22 N2 O15 N1 -150.6(3) 1_455 . . 1_455
N4 N2 O15 N1 -132.7(4) 1_455 . . 1_455
O13 N2 O15 N1 14.2(3) 1_455 . . 1_455
O20 N2 O15 N1 -134.7(5) 1_455 . . 1_455
O12 N2 O15 N1 1.4(3) 1_455 . . 1_455
O16 N2 O15 N3 -15.5(14) . . . .
O14 N2 O15 N3 165.7(6) . . . .
Lu2 N2 O15 N3 166.5(9) . . . .
O22 N2 O15 N3 -102.3(7) 1_455 . . .
N4 N2 O15 N3 -84.4(7) 1_455 . . .
O13 N2 O15 N3 62.5(7) 1_455 . . .
O20 N2 O15 N3 -86.3(8) 1_455 . . .
N1 N2 O15 N3 48.3(7) 1_455 . . .
O12 N2 O15 N3 49.8(8) 1_455 . . .
O16 N2 O14 Lu2 -178.0(8) . . . .
O15 N2 O14 Lu2 0.8(8) . . . .
O22 N2 O14 Lu2 -80.1(4) 1_455 . . .
N4 N2 O14 Lu2 -100.6(4) 1_455 . . .
O13 N2 O14 Lu2 78.0(5) 1_455 . . .
O20 N2 O14 Lu2 -118.9(3) 1_455 . . .
N1 N2 O14 Lu2 98.0(5) 1_455 . . .
O12 N2 O14 Lu2 116.6(3) 1_455 . . .
O16 N2 O14 N4 -77.5(9) . . . 1_455
O15 N2 O14 N4 101.4(8) . . . 1_455
Lu2 N2 O14 N4 100.6(4) . . . 1_455
O22 N2 O14 N4 20.4(3) 1_455 . . 1_455
O13 N2 O14 N4 178.5(6) 1_455 . . 1_455
O20 N2 O14 N4 -18.3(3) 1_455 . . 1_455
N1 N2 O14 N4 -161.4(7) 1_455 . . 1_455
O12 N2 O14 N4 -142.8(6) 1_455 . . 1_455
O16 N2 O14 N1 84.0(9) . . . 1_455
O15 N2 O14 N1 -97.2(9) . . . 1_455
Lu2 N2 O14 N1 -98.0(5) . . . 1_455
O22 N2 O14 N1 -178.1(6) 1_455 . . 1_455
N4 N2 O14 N1 161.4(7) 1_455 . . 1_455
O13 N2 O14 N1 -20.0(3) 1_455 . . 1_455
O20 N2 O14 N1 143.1(6) 1_455 . . 1_455
O12 N2 O14 N1 18.6(3) 1_455 . . 1_455
O16 N2 O14 N2 30.9(11) . . . 2_477
O15 N2 O14 N2 -150.3(6) . . . 2_477
Lu2 N2 O14 N2 -151.1(6) . . . 2_477
O22 N2 O14 N2 128.7(4) 1_455 . . 2_477
N4 N2 O14 N2 108.3(5) 1_455 . . 2_477
O13 N2 O14 N2 -73.2(6) 1_455 . . 2_477
O20 N2 O14 N2 90.0(4) 1_455 . . 2_477
N1 N2 O14 N2 -53.1(7) 1_455 . . 2_477
O12 N2 O14 N2 -34.5(6) 1_455 . . 2_477
O19 N3 O17 Lu3 -175.4(8) . . . .
O18 N3 O17 Lu3 -0.9(9) . . . .
O19 N3 O17 Lu3 -93.4(4) 2_466 . . .
N3 N3 O17 Lu3 -111.3(4) 2_466 . . .
O25 N3 O17 Lu3 -177.1(5) 1_455 . . .
O26 N3 O17 Lu3 -113(2) 2_466 . . .
O20 N3 O17 Lu3 106.0(5) 1_445 . . .
O17 N3 O17 Lu3 -111.3(4) 2_466 . . .
O19 N3 O17 N3 -64.1(9) . . . 2_466
O18 N3 O17 N3 110.4(9) . . . 2_466
Lu3 N3 O17 N3 111.3(4) . . . 2_466
O19 N3 O17 N3 17.9(3) 2_466 . . 2_466
O25 N3 O17 N3 -65.8(4) 1_455 . . 2_466
O26 N3 O17 N3 -2(2) 2_466 . . 2_466
O20 N3 O17 N3 -142.7(8) 1_445 . . 2_466
O17 N3 O17 N3 0.0000(10) 2_466 . . 2_466
O19 N3 O17 N4 101.4(13) . . . 1_445
O18 N3 O17 N4 -84.2(10) . . . 1_445
Lu3 N3 O17 N4 -83.3(8) . . . 1_445
O19 N3 O17 N4 -176.6(8) 2_466 . . 1_445
N3 N3 O17 N4 165.5(10) 2_466 . . 1_445
O25 N3 O17 N4 99.6(7) 1_455 . . 1_445
O26 N3 O17 N4 164(3) 2_466 . . 1_445
O20 N3 O17 N4 22.8(4) 1_445 . . 1_445
O17 N3 O17 N4 165.5(10) 2_466 . . 1_445
O19 N3 O17 N1 49.0(10) . . . 1_455
O18 N3 O17 N1 -136.6(7) . . . 1_455
Lu3 N3 O17 N1 -135.7(5) . . . 1_455
O19 N3 O17 N1 131.0(3) 2_466 . . 1_455
N3 N3 O17 N1 113.1(4) 2_466 . . 1_455
O25 N3 O17 N1 47.2(2) 1_455 . . 1_455
O26 N3 O17 N1 111(3) 2_466 . . 1_455
O20 N3 O17 N1 -29.6(7) 1_445 . . 1_455
O17 N3 O17 N1 113.1(4) 2_466 . . 1_455
O19 N3 O17 N2 15.3(15) . . . .
O18 N3 O17 N2 -170.3(7) . . . .
Lu3 N3 O17 N2 -169.3(10) . . . .
O19 N3 O17 N2 97.3(8) 2_466 . . .
N3 N3 O17 N2 79.4(9) 2_466 . . .
O25 N3 O17 N2 13.6(6) 1_455 . . .
O26 N3 O17 N2 78(3) 2_466 . . .
O20 N3 O17 N2 -63.3(11) 1_445 . . .
O17 N3 O17 N2 79.4(9) 2_466 . . .
O17 N3 O19 N3 78.6(9) . . . 2_466
O18 N3 O19 N3 -95.4(9) . . . 2_466
O19 N3 O19 N3 0.0000(10) 2_466 . . 2_466
O25 N3 O19 N3 80.7(4) 1_455 . . 2_466
O26 N3 O19 N3 -84.9(5) 2_466 . . 2_466
O20 N3 O19 N3 -165.0(4) 1_445 . . 2_466
O17 N3 O19 N3 -19.9(3) 2_466 . . 2_466
O17 N3 O19 N4 -134.1(9) . . . 1_445
O18 N3 O19 N4 51.8(9) . . . 1_445
O19 N3 O19 N4 147.2(4) 2_466 . . 1_445
N3 N3 O19 N4 147.2(4) 2_466 . . 1_445
O25 N3 O19 N4 -132.1(5) 1_455 . . 1_445
O26 N3 O19 N4 62.4(4) 2_466 . . 1_445
O20 N3 O19 N4 -17.7(3) 1_445 . . 1_445
O17 N3 O19 N4 127.4(4) 2_466 . . 1_445
O19 N3 O18 Lu3 175.4(8) . . . .
O17 N3 O18 Lu3 0.9(10) . . . .
O19 N3 O18 Lu3 84.4(4) 2_466 . . .
N3 N3 O18 Lu3 103.4(5) 2_466 . . .
O26 N3 O18 Lu3 166.7(5) 2_466 . . .
O20 N3 O18 Lu3 -127.6(4) 1_445 . . .
O17 N3 O18 Lu3 121.2(4) 2_466 . . .
O19 N3 O18 N4 -54.5(10) . . . 1_445
O17 N3 O18 N4 131.0(8) . . . 1_445
Lu3 N3 O18 N4 130.1(5) . . . 1_445
O19 N3 O18 N4 -145.5(3) 2_466 . . 1_445
N3 N3 O18 N4 -126.5(4) 2_466 . . 1_445
O26 N3 O18 N4 -63.2(2) 2_466 . . 1_445
O20 N3 O18 N4 2.5(3) 1_445 . . 1_445
O17 N3 O18 N4 -108.7(3) 2_466 . . 1_445
O19 N3 O18 N3 72.0(9) . . . 2_466
O17 N3 O18 N3 -102.5(9) . . . 2_466
Lu3 N3 O18 N3 -103.4(5) . . . 2_466
O19 N3 O18 N3 -19.0(3) 2_466 . . 2_466
O26 N3 O18 N3 63.3(5) 2_466 . . 2_466
O20 N3 O18 N3 129.0(5) 1_445 . . 2_466
O17 N3 O18 N3 17.8(3) 2_466 . . 2_466
O19 N3 O18 N4 6.2(15) . . . 2_566
O17 N3 O18 N4 -168.3(8) . . . 2_566
Lu3 N3 O18 N4 -169.3(11) . . . 2_566
O19 N3 O18 N4 -84.9(9) 2_466 . . 2_566
N3 N3 O18 N4 -65.9(10) 2_466 . . 2_566
O26 N3 O18 N4 -2.6(7) 2_466 . . 2_566
O20 N3 O18 N4 63.1(9) 1_445 . . 2_566
O17 N3 O18 N4 -48.1(9) 2_466 . . 2_566
O21 N4 O22 N2 -98.9(9) . . . 1_655
O20 N4 O22 N2 78.4(9) . . . 1_655
O16 N4 O22 N2 -1.9(4) 1_655 . . 1_655
O18 N4 O22 N2 158.0(6) 1_665 . . 1_655
O15 N4 O22 N2 -19.7(3) 1_655 . . 1_655
O19 N4 O22 N2 142.7(4) 1_665 . . 1_655
O5 N4 O22 N2 -23.9(13) . . . 1_655
O21 N4 O22 N3 118.7(9) . . . 1_665
O20 N4 O22 N3 -64.0(9) . . . 1_665
O16 N4 O22 N3 -144.3(4) 1_655 . . 1_665
N2 N4 O22 N3 -142.5(4) 1_655 . . 1_665
O18 N4 O22 N3 15.5(3) 1_665 . . 1_665
O15 N4 O22 N3 -162.2(5) 1_655 . . 1_665
O19 N4 O22 N3 0.2(3) 1_665 . . 1_665
O5 N4 O22 N3 -166.4(11) . . . 1_665
O21 N4 O22 N4 33.0(8) . . . 2_676
O20 N4 O22 N4 -149.7(9) . . . 2_676
O16 N4 O22 N4 130.0(4) 1_655 . . 2_676
N2 N4 O22 N4 131.8(4) 1_655 . . 2_676
O18 N4 O22 N4 -70.2(3) 1_665 . . 2_676
O15 N4 O22 N4 112.1(5) 1_655 . . 2_676
O19 N4 O22 N4 -85.5(3) 1_665 . . 2_676
O5 N4 O22 N4 107.9(11) . . . 2_676
O22 N4 O21 Lu4 177.2(9) . . . .
O20 N4 O21 Lu4 -0.3(9) . . . .
O16 N4 O21 Lu4 81.7(4) 1_655 . . .
N2 N4 O21 Lu4 100.3(4) 1_655 . . .
O18 N4 O21 Lu4 -109.9(4) 1_665 . . .
O15 N4 O21 Lu4 120.0(3) 1_655 . . .
O19 N4 O21 Lu4 -71.5(5) 1_665 . . .
O5 N4 O21 Lu4 44.0(2) . . . .
O22 N4 O21 N2 76.9(9) . . . 1_655
O20 N4 O21 N2 -100.6(9) . . . 1_655
Lu4 N4 O21 N2 -100.3(4) . . . 1_655
O16 N4 O21 N2 -18.6(3) 1_655 . . 1_655
O18 N4 O21 N2 149.8(7) 1_665 . . 1_655
O15 N4 O21 N2 19.7(2) 1_655 . . 1_655
O19 N4 O21 N2 -171.8(7) 1_665 . . 1_655
O5 N4 O21 N2 -56.3(5) . . . 1_655
O22 N4 O21 N4 -41.2(10) . . . 2_676
O20 N4 O21 N4 141.4(7) . . . 2_676
Lu4 N4 O21 N4 141.7(5) . . . 2_676
O16 N4 O21 N4 -136.6(4) 1_655 . . 2_676
N2 N4 O21 N4 -118.0(4) 1_655 . . 2_676
O18 N4 O21 N4 31.8(6) 1_665 . . 2_676
O15 N4 O21 N4 -98.4(4) 1_655 . . 2_676
O19 N4 O21 N4 70.2(5) 1_665 . . 2_676
O5 N4 O21 N4 -174.3(6) . . . 2_676
O22 N4 O21 N3 -94.0(11) . . . 1_665
O20 N4 O21 N3 88.6(9) . . . 1_665
Lu4 N4 O21 N3 88.9(5) . . . 1_665
O16 N4 O21 N3 170.6(7) 1_655 . . 1_665
N2 N4 O21 N3 -170.8(8) 1_655 . . 1_665
O18 N4 O21 N3 -21.0(3) 1_665 . . 1_665
O15 N4 O21 N3 -151.1(7) 1_655 . . 1_665
O19 N4 O21 N3 17.4(3) 1_665 . . 1_665
O5 N4 O21 N3 132.9(4) . . . 1_665
O22 N4 O21 N3 11.3(15) . . . 2_566
O20 N4 O21 N3 -166.1(7) . . . 2_566
Lu4 N4 O21 N3 -165.9(9) . . . 2_566
O16 N4 O21 N3 -84.1(8) 1_655 . . 2_566
N2 N4 O21 N3 -65.6(9) 1_655 . . 2_566
O18 N4 O21 N3 84.2(8) 1_665 . . 2_566
O15 N4 O21 N3 -45.9(9) 1_655 . . 2_566
O19 N4 O21 N3 122.7(7) 1_665 . . 2_566
O5 N4 O21 N3 -121.9(9) . . . 2_566
O22 N4 O20 Lu4 -177.2(8) . . . .
O21 N4 O20 Lu4 0.3(9) . . . .
O16 N4 O20 Lu4 -90.6(3) 1_655 . . .
N2 N4 O20 Lu4 -110.6(3) 1_655 . . .
O18 N4 O20 Lu4 120.8(3) 1_665 . . .
O15 N4 O20 Lu4 -112.5(4) 1_655 . . .
O19 N4 O20 Lu4 101.6(4) 1_665 . . .
O5 N4 O20 Lu4 -36.9(2) . . . .
O22 N4 O20 N2 -66.6(9) . . . 1_655
O21 N4 O20 N2 110.9(8) . . . 1_655
Lu4 N4 O20 N2 110.6(3) . . . 1_655
O16 N4 O20 N2 20.0(2) 1_655 . . 1_655
O18 N4 O20 N2 -128.5(4) 1_665 . . 1_655
O15 N4 O20 N2 -1.9(3) 1_655 . . 1_655
O19 N4 O20 N2 -147.8(3) 1_665 . . 1_655
O5 N4 O20 N2 73.7(3) . . . 1_655
O22 N4 O20 N3 64.4(9) . . . 1_665
O21 N4 O20 N3 -118.1(8) . . . 1_665
Lu4 N4 O20 N3 -118.4(4) . . . 1_665
O16 N4 O20 N3 151.0(3) 1_655 . . 1_665
N2 N4 O20 N3 131.0(3) 1_655 . . 1_665
O18 N4 O20 N3 2.4(3) 1_665 . . 1_665
O15 N4 O20 N3 129.1(4) 1_655 . . 1_665
O19 N4 O20 N3 -16.8(2) 1_665 . . 1_665
O5 N4 O20 N3 -155.3(3) . . . 1_665
